1.
MODELING AND SIMULATION OF HIGH PRESSURE COMPOSITE CYLINDERS FOR HYDROGEN STORAGE by JIANBING HU A DISSERTATION Presented to the Faculty of the Graduate School of the MISSOURI UNIVERSITY OF SCIENCE AND TECHNOLOGY In Partial Fulfillment of the Requirements for the Degree DOCTOR OF PHILOSOPHY IN MECHANICAL ENGINEERING 2009 Approved by K. Chandrashekhara, Advisor Lokeswarappa R. Dharani Hai-Lung Tsai Gregory E. Hilmas William E. Showalter
3.
iii PUBLICATION DISSERTATION OPTION This dissertation has been prepared in the form of three papers for publication asfollows:Pages 7-47 have been published in ADVANCED COMPOSITE MATERIALS.Pages 48-87 have been published in INTERNATIONAL JOURNAL OF HYDROGEN ENERGY.Pages 88-128 intended to submit to INTERNATIONAL JOURNAL OF HYDROGEN ENERGY.
4.
iv ABSTRACT Composite hydrogen cylinders provide an efficient means of storage of hydrogen gasfor modern hydrogen vehicles. Safety issues arising from the high gas pressure,temperature variation, fire attack, and fracture failures are the main concerns. The focusof this study is to develop a Finite Element (FE) model to predict the performance ofcomposite cylinders subjected to extreme mechanical/thermal loadings and provideguidance for design optimization. In the first part of this work, a predictive FE model ofcomposite cylinders has been developed considering various mechanical and thermalloadings. Doubly-curved laminated shell theory, accounting for transverse sheardeformation and geometric nonlinearity, is used to model the composite cylinder wall. Aback-propagation Neural Network (NNk) model, which is capable of predicting thefailure pressure for arbitrarily specified loading conditions, has been developed. Also, thefailure types and effects of thermal loading are investigated. In the second part, acomprehensive FE model has been developed to predict the behavior of the cylindersubjected to flame impingements. A failure model based on Hashin’s theory has beenimplemented to detect various failure modes of the composite. Damage due to resin burn-out and mechanical degradation are also considered in the model. Numerical results arepresented for thermal damage, residual properties and resin content profile of thecylinder. In the third part, fracture behavior of the cylinder with an axial surface crack inthe liner has been studied using fracture mechanics and a global-local FE technique withconsideration of autofrettage effect. Results on the fracture parameters (K and J-integral)with various autofrettage levels, crack sizes and crack shapes are presented.
5.
v ACKNOWLEDGMENTS The author wishes to extend his deepest gratitude to his academic advisor, Dr. K.Chandrashekhara, for his continued guidance, advice, encouragement and financialsupport throughout the course of the investigation and successful completion of thisdissertation research. The author also wishes to extend his greatest appreciation to the members of theadvisory committee, Dr. Lokeswarappa. R. Dharani, Dr. Hai-Lung Tsai, Dr. Gregory E.Hilmas, and Dr. William E. Showalter for their advice and encouragement, and their timeand effort for review of this dissertation. Many thanks go to Dr. S. Sundararaman for his prior input in this research. Theauthor also appreciates the assistance from his fellow colleagues and friends, Mr. JianChen, Mr. V.G.K. Menta and Mr. R. Vuppalapati. The author would like to take this opportunity to thank Mr. William Chernicoff of theUS Department of Transportation for his assistance with information and ideas. Thefunding of this research by the US Department of Transportation is gratefullyacknowledged. The author would also like to acknowledge the financial support received from theDepartment of Mechanical and Aerospace Engineering at Missouri S&T for GraduateResearch Assistantship and Graduate Teaching Assistantship. Finally, the author wishes to express his deepest gratitude to his parents, his sistersand brothers-in-law for their understanding, patience, encouragement, support, and forhelping realize and accomplish his dreams.
6.
vi TABLE OF CONTENTS PagePUBLICATION DISSERTATION OPTION ................................................................ iiiABSTRACT ..................................................................................................................ivACKNOWLEDGMENTS ..............................................................................................vLIST OF ILLUSTRATIONS .........................................................................................ixLIST OF TABLES ........................................................................................................xiSECTION1. INTRODUCTION ......................................................................................................11.1. BACKGROUND .....................................................................................................11.2. SCOPE AND OBJECTIVES ...................................................................................31.3. CONCLUDING REMARKS ..................................................................................5PAPER I. FAILURE PRESSURE PREDICTION OF COMPOSITE CYLINDERS FOR HYDROGEN STORAGE USING THERMO-MECHANICAL ANALYSIS AND NEURAL NETWORK ...........................................................................................7 ABSTRACT ..........................................................................................................7 1. INTRODUCTION .............................................................................................8 2. SHEAR DEFORMABLE SHELL THEORY ...................................................10 3. COMPOSITE FAILURE MODEL ...................................................................13 4. MATERIAL PROPERTIES .............................................................................14 5. FINITE ELEMENT SIMULATION .................................................................15 6. NEURAL NETWORK MODEL ......................................................................17 7. RESULTS AND DISCUSSION .......................................................................19 8. CONCLUSIONS .............................................................................................22 REFERENCES ....................................................................................................23 II. ANALYSIS OF COMPOSITE HYDROGEN STORAGE CYLINDERS SUBJECTED TO LOCALIZED FLAME IMPINGEMENTS ..............................48 ABSTRACT .......................................................................................................48 1. INTRODUCTION ..........................................................................................49 2. MODELING OF HIGH PRESSURE COMPOSITE HYDROGEN STORAGE CYLINDERS ..................................................................................................51
7.
vii 2.1. Thermal Model .........................................................................................51 2.2. Sub-laminate Model .................................................................................53 2.3. Formulation of Finite Element Model .......................................................55 3. MATERIAL MODELS ....................................................................................56 3.1. Temperature Dependent Material Properties .............................................56 3.2. Composite Failure Criteria ........................................................................57 3.3. Model for Hydrogen Gas ..........................................................................58 4. FINITE ELEMENT SIMULATION PROCEDURE .........................................59 5. RESULTS AND DISCUSSION .......................................................................60 6. CONCLUSIONS .............................................................................................62 REFERENCES ....................................................................................................63III. FRACTURE ANALYSIS OF HYDROGEN STORAGE COMPOSITE CYLINDERS WITH LINER CRACK ACCOUNTING FOR AUTOFRETTAGE EFFECT .............................................................................................................88 ABSTRACT .......................................................................................................88 1. INTRODUCTION ...........................................................................................89 2. METHODOLOGY ..........................................................................................91 2.1. Autofrettage Effect on High Pressure Composite Cylinder for Hydrogen Storage .....................................................................................................91 2.2. Stress Intensity Factor (K) Evaluation .......................................................93 2.3. J-Integral Evaluation ................................................................................94 2.4. Material Models ........................................................................................95 3. FINITE ELEMENT SIMULATION ...............................................................97 3.1. Global Model ............................................................................................98 3.2. Local Model .............................................................................................99 3.3. Simulation Procedure ..............................................................................100 4. RESULTS AND DISCUSSION .....................................................................101 4.1. Autofrettage Process Simulation ............................................................101 4.2. Stress Intensity Factor (K) and J-integral ...............................................102 4.3. Stress Field Characterization on the Crack Tip Vicinity .........................103 5. CONCLUSIONS ..........................................................................................104 REFERENCES .................................................................................................105
9.
ix LIST OF ILLUSTRATIONSFigure PagePAPER I1. Structure scheme of hydrogen storage cylinder .........................................................342. Doubly curved shell and coordinate system ...............................................................353. Finite element model of hydrogen cylinder ...............................................................364. Feedforward back-propagation Neural Network architecture .....................................375(a). Uniform thermal loading with Tin=Tout (in Case 1) ................................................385(b). Uniform thermal loading Tin=Tout (in Case 2) .......................................................395(c). Uniform thermal loading Tin=Tout (in Case 3) .......................................................406(a). Gradient thermal loading with Tout=50oC (in Case 1) ............................................416(b). Gradient thermal loading with Tout=50oC (in Case 2) ............................................426(c). Gradient thermal loading with Tout=50oC (in Case 3) ............................................437. Failure pressure with inside temperature variation (Tout=25oC) ..................................448. Ply-by-ply failure predictions under various thermal loadings ...................................459(a). Comparison of failure pressures from NNk and ABAQUS at = 15o ...................469(b). Comparison of failure pressures from NNk and ABAQUS at = 25o ...................47PAPER II1. Schematic of hydrogen cylinder ................................................................................732. Curve fitting for hydrogen gas state equation at constant density ...............................743. Finite element model of the cylinder .........................................................................754. Stacking sequence of the cylinder wall ......................................................................765. Finite element implementation schemes ....................................................................776. Variation of sink temperature with film coefficient ...................................................787. Internal pressure variation with time for various flame area sizes ..............................798. Temperature distributions along the length at inner surface of the aluminum liner .....809. Temperature distributions through composite thickness ............................................8110. Residual resin content through the thickness ...........................................................8211. Stress (S11) distribution through the thickness .........................................................8312. Stress (S22, S33) distribution through the thickness ...................................................8413(a). Fiber fracture index (Imt) contour around heat source ..........................................85
10.
x13(b). Matrix cracking index (Ift) contour around heat source .......................................8613(c). Density index (ρ/ρ0) contour around heat source .................................................87PAPER III1. Schematic of hydrogen composite cylinder .............................................................1122. Diagram of autofrettage process ..............................................................................1133. Schematic of domain integral evaluation .................................................................1144. Global finite element model ....................................................................................1155. Local finite element model ......................................................................................1166. Implementation scheme ..........................................................................................1177. von-Mises stress distribution in liner .......................................................................1188. Cyclic stress-strain curves for various autofrettage levels ........................................1199. Stress intensity factor (K) along crack front for various autofrettage levels .............12010. J-integral along crack front for various autofrettage levels ....................................12111. Stress intensity factor (K) against pressure loading for various autofrettage levels 12212. J-integral against pressure loading for various autofrettage levels ..........................12313. Stress intensity factor (K) along crack front with various geometric ratios ............12414. J-integral along crack front with various geometric ratios ......................................12515. Stress distribution of the crack front vicinity .........................................................12616. Transition of plastic zone shapes along crack front ................................................12717. Plastic zone shapes for various autofrettage levels .................................................128
11.
xi LIST OF TABLESTable PagePAPER I1. Ultimate strength of carbon/epoxy composite ...........................................................272. Mechanical and thermal properties of S-glass/epoxy .................................................283. Mechanical and thermal properties of Aluminum Alloy 6061-T6 ..............................294. Lay-up configurations for various winding patterns ..................................................305. Weights and biases for trained neural network ..........................................................316. Scale constants for trained neural network ................................................................327. Testing cases and maximum error of prediction ........................................................33PAPER II1. Curve fitting parameters for transverse and shear modulus ........................................672. Thermal expansion coefficients of carbon/epoxy .......................................................683. Specific heat and thermal conductivity of carbon/epoxy ............................................694. Parameters for resin reaction model ..........................................................................705. Strength of carbon/epoxy ..........................................................................................716. Design parameters for the cylinder ............................................................................72PAPER III1. Mechanical properties of carbon/epoxy composite ..................................................1102. Mechanical properties of Aluminum Alloy 7075-T651 ...........................................111
12.
1. INTRODUCTION1.1. BACKGROUND Currently, the energy crisis and environmental pollution arising from burning fossilfuel in vehicles are identified as some of the major concerns in the global world.Hydrogen, a renewable and clean energy resource, is a promising substitute for fossilfuels. One of the key challenges for the usage of hydrogen gas in automobiles is todevelop a compact and efficient way of hydrogen storage. The solutions for thischallenge can be categorized into three main groups [1-2]: (a) Cryogenic hydrogenstorage: It provides high volumetric density (0.07 kg/L) and good weight density (2.8 %),but liquefaction (-423.2 oF) is an intensive energy consuming process and evaporationreduces the gas usage efficiency. (b) Hydrogen storage materials: Traditional metallichydrogen storage materials provide a safe way to store hydrogen gas, but a low weightdensity (1.4 %) and operation complexity prohibit it from practical applications.Recently, carbon nano-tubes have attracted much research interest as a future hydrogenstorage material, but it still remains in the early investigation phase [3]. (c) Compressedhydrogen gas: It is expected to be the main stream for hydrogen storage in the near futureas it provides good volumetric and weight density (0.03 kg/L and 6%) and simplicity oftransportation and storage. Traditionally, compressed hydrogen gas is stored in metallic cylinders (Type Icylinder). The storage pressure for this type of cylinder is low (usually less than 25 MPa)and the capacity of hydrogen gas storage is limited. Also, hydrogen embrittlement canresult in micro-cracks and reduce the strength of the cylinder. The Type II cylinder isdeveloped by wrapping fiber-reinforced composite materials in the hoop direction on themetallic cylinder [4]. It reduces the weight of the cylinder significantly. However, thisstill does not meet the requirement of hydrogen storage capacity for automotives. Tofurther reduce the weight and increase the storage capacity, fully wrapped compositecylinders (Type III and Type IV) have been introduced. The cylinders are manufacturedby the filament winding technique. In this process, a liner is used as a mandrel and thehigh strength, low density composite (fiber strength 5-6 GPa, composite density 1.6g/cm3) is fully wrapped in both the helical and the hoop directions. The helical winding
13.
2produces helical layers to bear the axial loading, while the hoop winding generates hooplayers to carry circumferential loading. The liner serves as a gas barrier after the cylinderis manufactured. The Type III differentiates the Type IV by the material used for the liner(aluminum for Type III and polymer for Type IV). To obtain efficient storage capacity,the cylinders are designed for pressures as high as 5,000 to 10,000 psi and, hence, thefailure of the cylinder would lead to a catastrophic accident. In this context, safeinstallation and operation of high-pressure composite cylinders for hydrogen storage areof primary concern. To design the cylinder with the highest possible safety, reliabilityand minimum weight considerations, mechanics relevant to the behavior of the cylindermust be well understood. The early technique used for analyzing filament-wound composite cylinders is nettinganalysis [5-7]. This procedure has been widely used in the industry for its simplicity. Astatic equilibrium principle is applied to obtain the stress on the fiber by neglecting thecontribution of the resin matrix. Although this technique provides a concise way topredetermine some design parameters for cylinder prototypes, more detailed analysis isnecessary for examining and optimizing the high pressure composite cylinder forhydrogen storage under various operating conditions. Considering the effect of resin matrix, many studies have been focused on developingan analytical solution for composite cylinders under various loadings. Lekhnitskii [8] laidthe foundation for analyzing the anisotropic elasticity. Numerous authors [9-13]advanced the model for the stress analysis of cylinders under uniaxial, biaxial andcombined centrifugal pressure loadings in terms of stress functions. Later on, based on aplain-strain assumption, Akcay and Kaynak [14] analyzed closed-end cylinders underuniform thermal loading. Sayman [15] incorporated a general hydrothermal effect in themodel that is suitable for multi-layered thin/thick composite cylinders for the axiallysymmetric case under uniform or parabolic temperature distributions. Tabakov [16]developed a model to obtain exact solutions for the thick laminated anisotropic cylinderwith closed ends, but this model was limited to five layers and was not universal. In hislater work [17], a general model was developed by deriving the governing differentialequations instead of stress functions without considering the end effects and closing
14.
3plates. More recently, Chapelle and Perreux [18] extended the analytical method toanalyzing a Type III hydrogen cylinder by including plastic flow of the liner. The Finite Element Method (FEM) provides a convenient tool to analyze compositecylinders with consideration of nonlinearities, failure modes and various loadingconditions. A three dimensional finite element was developed by Hoa et al. [19] for thestrain analysis of fiber reinforced plastic vessels containing discontinuities such asmanhole connections or nozzles. Considering the change of winding angles through thethickness of helical laminates, finite element analyses were performed by Park et al. [20]through coding the winding angle to each solid element. Kabir [21] modeled the structureof the cylinder wall as an elastic, ideally plastic liner, reinforced with quasi-isotropicelastic composite. Tam et al. [22] analyzed the composite tank considering both materialand geometric nonlinearities. Gray and Moser [23] described a method which has beendeveloped to analyze filament-wound composite pressure vessels accounting for thehighly orthotropic nature of vessel structures. Kim et al. [24] employed a 3-D element tocompute stresses for optimizing the composite pressure vessel design. In addition,significant studies were conducted by several researchers [25-28] on the analysis ofcomposite pressure vessels with incorporating failure and progressive damage models inFE programs. The fracture and fatigue behavior of composite pipes and cylinders havealso been investigated by many authors [29-34] using both stress/strain criteria and directcrack-modeling techniques in finite element models.1.2. SCOPE AND OBJECTIVES Based on the literature survey, many researchers have used finite element method onthe study of composite vessels or pipes, but there is no significant research on theanalysis of Type III cylinders subjected to thermo-mechanical loading. In the case of fireimpingements, the previous studies have been carried out on flat composite panels andlack the capability of analyzing composite cylinders considering both mechanical andthermal damage. Furthermore, fracture failure is another essential factor for the safetyand design life-expectancy of the cylinder. Most of the previous studies have performedfracture analysis either on compressed natural gas cylinders or on pressure vessels usedfor aerospace. Intensive analysis has been conducted on metallic cylinders and a few are
15.
4related to cylinders with a metallic liner wrapped by composites. However, not muchresearch has been performed on composite hydrogen cylinders with consideration of theautofrettage effect. As an effort to develop the finite element model to predict the behavior of Type IIIhydrogen cylinders for the safety concern and design guidance, this study focuses onthree aspects. The first one is to develop a finite element model that can predict thefailure pressure of the cylinder subjected to combined thermal and mechanical loadings.The second one is to develop a comprehensive finite element model that can identifyfailure modes of the cylinder when it is attacked by fire impingement. The third one is toevaluate the performance of the cylinder containing liner cracks from the perspectiveview of fracture mechanics using finite element simulation technique. This dissertation has been prepared in the form of three parts corresponding to theaddressed problems. The first part is titled “Failure Pressure Prediction of Composite Cylinders forHydrogen Storage using Thermo-mechanical Analysis and Neural Network.” In thispart, a finite element simulation tool for the design of hydrogen storage cylinders hasbeen developed. The structural response of the cylinder is analyzed using laminated shelltheory accounting for transverse shear deformation and geometric nonlinearity. Acomposite failure model is used to evaluate the failure pressure. A back-propagationNeural Network model is developed based on the results of finite element analysis topredict the maximum failure pressure for arbitrary thermo-mechanical loading conditions. The second part is titled “Analysis of Composite Hydrogen Storage CylindersSubjected to Localized Flame Impingements.” In this part, a comprehensive non-linearfinite element model has been developed for predicting the behavior of compositehydrogen storage cylinders subjected to high pressure and localized flame impingements.The model is formulated in an axi-symmetric coordinate system and incorporates varioussub-models to capture the behavior of the composite cylinder under extreme thermo-mechanical loadings. Sub-models are implemented in ABAQUS commercial finiteelement code using user subroutines. Numerical results are presented for thermal damage,residual properties and profile of resin content of the cylinder wall.
16.
5 The third part is titled “Fracture Analysis of Hydrogen Storage CompositeCylinders with Liner Crack accounting for Autofrettage Effect.” In this part, aglobal-local finite element model is developed to investigate the axial surface flaws in theliner of high pressure composite cylinders for hydrogen storage using fracture mechanics.The effect of autofrettage process is studied due to its strong influence on the cylinderfracture behavior. The autofrettage process simulation is conducted in the global model.The local model, which is driven by the results of the global model, performs a detailedanalysis of the crack to assure accurate computation of fracture parameters. Results ofboth stress intensity factor (K) and J-integral are reported along the crack front in fourautofrettage levels and with different crack sizes. The plastic zone along the crack front isalso studied.1.3. CONCLUDING REMARKS In the first part, a doubly curved shell model accounting for transverse sheardeformation is used for the thermo-mechanical analysis of hydrogen composite storagecylinders. Temperature dependent material properties of the load carrying carbon/epoxylayer and geometry nonlinearity are also considered in the numerical model. Underuniform thermal loading, a temperature increase significantly raises the maximum failurepressure based on the Tsai-Wu failure criterion. Contrastively, the non-uniform thermalloading can cause an uneven load distribution and hence decrease the maximum failurepressure. The thickness ratio also plays an important role in determining the maximumfailure pressure and should be selected appropriately based on the thermal andmechanical loading conditions. A neural network model is developed and used to predictthe failure pressure. The performance of the trained neural network is then evaluated bycomparing the predicted values with those of testing cases. The results are in goodagreement. In the second part, a comprehensive finite element model has been developed toanalyze composite hydrogen storage cylinders subjected to high pressure and flameimpingements. The model considers the resin reaction, heat exchange between thehydrogen gas and liner, and the progressive failure process. A sub-laminate model hasbeen developed to reduce computational time. A temperature dependent material model
17.
6along with a failure model has been developed and implemented to accurately predictvarious failure modes for the hydrogen storage cylinder. Analysis of a typical highpressure composite hydrogen cylinder under fire exposure is conducted by using thedeveloped models. Parametric studies are done on heat exchange rate (between hydrogengas and the liner) and the size of the flame source. Stresses, temperature profile andfailure types are reported. The developed model can be used to accommodate varioustypes of thermal and mechanical loadings, lamina stacking sequence, and laminathickness to establish safe working conditions and design limits for hydrogen storagecylinders. In the third part, a global-local finite element model has been developed to predict thefracture behavior of high pressure composite cylinders for hydrogen storage. Simulationof the autofrettage process is carried out in the global model. Plastic hardening and theBauschinger effect are observed in the results. Both stress intensity factor (K) and J-integral are computed along the crack front in the local model with consideration ofautofrettage influence and crack size effect. It is found that the autofrettage processsignificantly improves the cylinder fracture performance and the smaller crack sizereduces the value of fracture parameters dramatically. The plastic zone around the cracktip is studied in terms of shape and size. The fracture behavior is discussed throughobservation of the plastic zone and the corresponding selection of parametriccharacterization is suggested. The current research can be extended in several ways for future work. The developedNeural Network model for failure pressure prediction can be applied to optimization ofcomposite lay-ups under arbitrary environmental temperature conditions. The second partof the model can be extended to multi-physics analysis by simulating the fluid field ofhydrogen gas in the cylinder. Pressure release device can be designed based on theprediction of simulation to minimize the hazard of cylinder failure when subjected toaccidental fire. The fracture model can be used as a tool for cylinder autofrettage processto obtain an optimum stress state to restrict crack growth in the liner. Also, the currentlydeveloped fracture model can be extended to predict the fatigue life of the cylinder andprovide guidance for material selection and lay-up optimization of the composite wall toachieve premium fracture performance.
18.
7 PAPER I: FAILURE PRESSURE PREDICTION OF COMPOSITE CYLINDERS FOR HYDROGEN STORAGE USING THERMO-MECHANICAL ANALYSIS AND NEURAL NETWORK ABSTRACT Safe installation and operation of high-pressure composite cylinders for hydrogenstorage are of primary concern. It is unavoidable for the cylinders to experiencetemperature variation, and significant thermal input (or flux) during the service. Themaximum failure pressure that the cylinder can sustain must be affected due to the natureof temperature dependent composites, integrity of the matrix and fibers and complexityof the cylinder design. Most of the analysis reported in high-pressure composite cylindersis based on simplified assumptions and does not account for complexities like thermo-mechanical behavior and temperature dependent material properties. In the present work,a comprehensive finite element simulation tool for the design of a hydrogen storagecylinder is developed. The structural response of the cylinder is analyzed using laminatedshell theory accounting for transverse shear deformation and geometric nonlinearity. Acomposite failure model is used to evaluate the failure pressure under various thermo-mechanical loadings. A back-propagation Neural Network (NNk) model is developed topredict the maximum failure pressure using the analysis results. The failure pressurespredicted from the NNk model are compared with those from testing cases. Thedeveloped NNk model is capable of predicting the failure pressure for any given loadingcondition.
19.
81. INTRODUCTION Composite high-pressure cylinders have potential application as hydrogen storagesystems in automotive, transportation, portable, and stationary storage systems due totheir light weight, simplicity of the storage and low cost for storage and transport ofhydrogen gas [1]. Typically, a composite high-pressure cylinder is made of a highmolecular weight polymer or aluminum liner that serves as a hydrogen gas permeationbarrier. A filament-wound, carbon/epoxy composite laminate over-wrapped outside ofthe liner provides the desired pressure load bearing capacity [2]. A vehicle fuel systemcylinder is capable of sustaining pressures of 5,000 psi or higher by taking advantage ofthe high strength and low specific weight of modern high performance composites. Inaddition, the maturation of the filament winding manufacturing process further reducesthe price to being practical and common for use in mass transportation systems. To design composite high-pressure cylinders with the highest possible safety,reliability and minimum weight considerations, the behavior of composite structuresunder various mechanical and thermal loadings, including localized and non-localizedflames, needs to be well understood. Studies have been conducted by various researchers[3-5] on the structure of hydrogen composite cylinders under mechanical loadings. Usingfinite element method as a powerful numerical tool, numerous studies have beenconducted on high-pressure cylinder analysis [6-8]. Compared to pure mechanicalloading, fewer studies have been conducted on hydrogen composite cylinders subjectedto thermal loads and combined thermo-mechanical loads [9, 10]. In the present study, a thermo-mechanical finite element model has been developedfor the analysis of hydrogen storage cylinders. The composite laminate wall of hydrogen
20.
9composite cylinder typically consists of helical and hoop laminated layers. Both theselayers, along with an aluminum liner, are considered for the analysis. During service,hydrogen composite cylinders unavoidably experience various thermal loadingscombined with high inner pressure. To account for working temperature variation in theservice, uniform temperature loadings ranging from 25C to 140 C are considered for theanalysis, above which the matrix begins to burn. During the gas filling process, the innertemperature can go up to around 100 C [10]. Hence, non-uniform thermal loadings havealso been included in the study. The variation of material properties with temperature issignificant for most composites. A temperature dependent material model has beendeveloped and implemented in commercial finite element code ABAQUS, using usersubroutines. A laminated shell theory [11, 12] accounting for out-of-plane shear strainsand geometric nonlinearity is used for the analysis. When considering the combination of various thermal loadings, winding angles andlay up configurations in the analysis, it is a tremendous task to optimize the cylinderdesign and predict maximum failure pressure through case-by-case simulation. A back-propagation Neural Network (NNk) model is then developed to predict the failurepressure using the results from a few typical finite element simulation cases. The trainingprocess consists of training the network with three sets of simulation results with variouswinding angles and thermal loadings. Once trained, the developed NNk model can beused for guidance and optimization of hydrogen cylinder design. Some testing cases,which are not included in the training sets, are utilized to compare with the predictedfailure pressure from the NNk model. A good agreement is found between failurepressures from testing cases and NNk model prediction.
21.
102. SHEAR DEFORMABLE SHELL THEORY A schematic of a hydrogen composite cylinder wall is shown in Figure 1. The innerliner is made of high molecular weight polymer or aluminum that serves as a hydrogengas permeation barrier. A filament-wound, carbon/epoxy composite laminate over-wrapped on the outside of the liner provides the desired pressure load bearing capacity[13]. In many current designs, a glass/epoxy layer is placed over the carbon/epoxylaminate to provide impact and damage resistance. The doubly curved shell theoryaccounting for out of plane shear deformations and geometric nonlinearity is used for theanalysis of composite hydrogen storage cylinders. A multilayered doubly curved shell is shown in Figure 2. The curved coordinatedsystem 1 , 2 , is used in space description. The coordinates 1 and 2 specify theposition on the middle surface, while measures the distance, along the outward normal,from the mid-surface to an arbitrary point on the shell. The displacement field can bewritten as: u( 1 , 2 , ) = (1 + ) u o ( 1 , 2 ) + 1 ( 1 , 2 ) (1.a) R1 v( 1 , 2 , ) = (1 + ) v o ( 1 , 2 ) + 2 ( 1 , 2 ) (1.b) R2 w ( 1 , 2 , ) = w o ( 1 , 2 ) (1.c)The non-linear strain-displacement relations based on Sanders’s shell theory can be givenas: o o εx= εx + ζ κ x ; εy = εy + ζ κ y o o o γ xy = γ xy + ζ κ xy ; γ yz = γ yz ; γ xz = γ xz (2)
22.
11where ε 0 and κ j are defined as: j 2 1 uo 1 w o 1 1 o ε = x + wo + 2 ; κx = α1 ξ1 R 1 2α1 ξ1 α1 ξ1 2 1 v 0 w 0 o 1 w o 1 2 ε y + 2 ; κy α 2 2 R 2 2α 2 ξ 2 α 2 2 1 vo 1 uo 1 w o w o 1 wo o γ xy = + + ; γo = yz + 2 - vo (3) α1 ξ1 α 2 ξ 2 2α1α 2 ξ1 ξ 2 α2 ξ 2 R2 1 w o o γ xz = + 1 - u o α1 ξ1 R1 1 2 1 1 1 vo 1 u o κ xy = + - co - α1 ξ1 α2 ξ 2 α1 ξ1 α 2 ξ 2 1 1 1 c0 = - ; dx = α1dξ1 ; dy = α 2 dξ 2 2 R1 R 2 In Eq. (3), u and v are the displacements in the direction of the tangents to the coordinatelines 1 and 2 , respectively, w is the displacement in the direction of the outwardnormal and 1 and 2 are the rotations. The stress-strain relation, accounting for thermal effects, in the shell coordinates for ak th layer can be expressed as [12]: x Q11 Q12 Q16 0 0 ε x xT Q Q Q26 0 0 ε y yT y 12 22 xy Q16 Q26 Q66 0 0 xy xyT (4) 0 0 0 Q44 Q45 yz yz xz k 0 0 0 Q45 Q55 k xz kwhere Qij are the transformed elastic coefficients, T is the given temperature distribution,and x , y , xy are the thermal expansion coefficients in the shell coordinates.
23.
12 The laminate constitutive equations can be obtained by integrating Eq. (4) over thethickness, and is written as: Nx A11 A12 A16 0 0 B11 B12 B16 ε0 NT x x N A 0 T y 12 A 22 A 26 0 0 B12 B22 B26 εy Ny N xy A16 A 26 A66 0 0 B16 B26 B66 γ0 NT xy xy 0 Q xz 0 0 0 A 44 A 45 0 0 0 γ xz 0 0 0 - (5) Q yz 0 0 A 45 A55 0 0 0 γ yz 0 Mx B11 B12 B16 0 0 D11 D12 D16 κx MT x B T My B22 B26 0 0 D12 D 22 D26 κy My 12 M xy κ MT B16 B26 B66 0 0 D16 D 26 D66 xy xy where N T and M T are thermal stress and moment resultants h/2 A ij Bij Dij h/2 Qij 1 z z 2 dz i, j 1, 2, 6 (6.a) h/2 Aij K i K j Qij dz i, j 4,5 (6.b) h/2 T T Nx , M x Q11 Q12 Q16 x T T h/2 N y , M y h / 2 Q12 Q22 Q26 y 1, z Tdz (6.c) N T , M T Q16 Q26 Q66 xy xy xy where K is a shear correction factor. Following the standard finite element procedure, the generalized displacements in anyelement are given by: u u v v N w w i (7) i 1 1 1 2 2 i where N is the number of nodes in the element and i are the interpolation functions.Substituting Eq. (7) in Eq. (3), the strains can be expressed as:
24.
13 B1 ; B2 ; B3 (8)The finite element equation is written as: K e e F e FTe (9)where , T T T K e B1T AB1 B1T BB2 B2 BB1 B2 DB2 B3 SB3 d ( Area ) T u v w e 1 2 F B e T 1 T N B2 M d ( Area) F B T e T 1 N T B2 M T d ( Area) TFor any given mechanical and temperature loadings, Eq. (9) can be assembled and solvedto determine displacements and stresses.3. COMPOSITE FAILURE MODEL The Tsai-Wu failure criterion is used for failure evaluation of hydrogen compositestorage cylinders [14]. Taking 1 as the fiber direction and 2 and 3 as transversedirections, the Tsai-Wu failure criterion can be expressed as: 2 2 2 I F F1 11 F2 22 F11 11 F22 22 F44 23 2 2 (10) F55 13 F66 12 2 F12 11 22 1.0The coefficients in Eq. (10) are defined as: 1 1 1 1 1 F1 , F2 , F11 , Xt Xc Yt Yc Xt Xc 1 1 1 1 F22 , F44 2 , F55 2 , F66 2 , YtYc S 23 S13 S12
25.
14 1 1 1 1 1 1 1 2 F12 2 1 biax biax 2 biax X t X c Yt Yc X t X c YtYc or F12 f F11F22 ( 1 f 1 )where, X t and X c are tensile and compressive stress strengths along the fiber direction,Yt and Yc are tensile and compressive stress strengths in the transverse fiber direction,S 23 , S13 and S12 are the maximum shear strengths in corresponding planes, biax is theequi-biaxial stress at failure and f is an experience coefficient.4. MATERIAL PROPERTIES Mechanical and thermal properties of fiber reinforced composites vary significantlywith temperature. As the carbon/epoxy laminate carries the pressure loading from thehydrogen gas, the effect of temperature on its material properties cannot be ignored. Themoduli and thermal expansion coefficients are dependent on temperature. For HFGCU125 carbon/epoxy, the temperature dependent material properties are given by [15]: E1= 0.066 T + 128 (GPa) (25C < T < 140C) E2 = 0.064 T + 10.67 (GPa) (25C < T < 140C) G12 = 0.034 T + 5.39 (GPa) (25C < T < 140C) (11) 12 = 0.0005 T + 0.44 (25C < T < 140C) α1= (0.0003 T2 0.04 T + 2.09) × 10-6 (25C < T < 140C) α2 = (0.0041 T2 0.23 T + 32.2) ×10-6 (25C < T < 140C)
26.
15 Furthermore, G13 is taken as G12, and G23 is assumed as 0.7G12. The ultimatestrengths of carbon/epoxy do not change much with this temperature range and areassumed to be constant and are listed in Table 1. The material properties for glass/epoxyare listed in Table 2. The outer most glass/epoxy layer is primarily used for protection ofthe load bearing carbon/epoxy lamina. Hence temperature dependent material propertiesare not used for the glass/epoxy layers. Properties of the innermost aluminum liner arelisted in Table 3.5. FINITE ELEMENT SIMULATION ABAQUS is an integrated and open-ended Finite Element Analysis code, which iswidely used by the industry as well as researchers for the flexibility of implementing userdefined subroutines and its powerful nonlinear solver. With those features, the userdefined problem can be built up by combination of the basic frames provided by theABAQUS code and user model specialties implementing subroutines. All the modelingfeatures described in this work have been thus implemented in this code. A laminatedshell element, based on doubly curved shell theory, accounting for membrane, bendingand membrane-bending coupling and transverse shear effects, is suitable for modelingboth thin and thick laminated composites. For this purpose, the laminated composite wallof the cylinder is modeled by using a doubly curved 8-node shell element (S8R). In orderto estimate the failure pressure of the cylinder, it is necessary to include a failurecriterion. Tsai-Wu failure theory is utilized to check and report the ply-by-ply laminatefailure by using a user subroutine UVARM. In addition, the temperature dependentmaterial properties are incorporated in the model by using subroutine USDFLD so that, at
27.
16each integration point, the material properties are determined by the given temperature.The orientation of each element at every ply is handled by subroutine ORIENT accordingto the winding pattern. The cylinder is modeled and meshed using the ABAQUS/CAEpreprocessor as shown in Figure 3. Due to the symmetry, 1/8th of the cylinder isconsidered for the analysis. The comprehensive model is then solved by using theABAQUS/standard solver with geometric nonlinearity considered. The dimensions considered in the present cylinder analysis are based on a typicaldesign from the literature [13]. The outer radius of the cylinder is taken as Rout = 0.25 mand the inner radius Rin = 0.22 m (Figure 1). The pressure bearing carbon/epoxy laminateconsists of 24 plies resulting in a composite shell of thickness 28 mm. The protectiveglass/epoxy layer and liner are 2 mm and 2.5 mm thick respectively. The cylinder issubjected to an internal pressure that gradually increases until failure occurs in the firstply. To manufacture closed cylinders, two types of winding patterns are usually used:hoop and helical/polar windings. The thickness ratio R (total thickness of helicallaminate/total thickness of hoop laminate) affects the failure pressure of the cylinder anda range of 0.1 to 2.0 is studied. The winding angle of laminae also affects the failurepressure of the cylinder and a range of 10◦ to 30◦ for helical winding and 89o for hoopwinding has been considered based on manufacturing feasibility. The plies in theprotection laminate are oriented as 45 angle ply.
28.
176. NEURAL NETWORK MODEL A feedforward back-propagation Neural Network (NNk) is used to predict the failurepressure of a hydrogen cylinder. A schematic of the NNk is shown in Figure 4. Therelationship of failure pressure and the inputs (thickness ratio R , temperature inside thecylinder Tin , temperature outside the cylinder Tout , and winding angle ) is modeled by atwo-layer (hidden layer and output layer) network. Each layer consists of a number ofprocessing units, with an activation function, known as neurons. For faster training and Trobust NNk, inputs are scaled to a desirable range by a designed transfer function finbefore entering the input layer. Inputs are passed through weighted connections to thehidden layer and then to the output layer. The output P is, finally, scaled back to failure Tpressure P by a designed transfer function f out . The number of neurons in the hiddenlayer and the characterizing weights and biases in the model are determined by trainingthe NNk. The input transfer function T fin ( I i ) I i ai bi (12)whereI i are input variables ( i 1, 2,3and 4 corresponding to R, Tin , Tout and respectively) n nai max min Iimax I imin bi nmin Min{ai I i }[ nmin nmax ] is the desired scale range and is taken as [-1 1] and I i are input training pattern vectors.
29.
18 Normalized input variables I i are given by T I i fin ( Ii ) (13) The activation function in the hidden layer is the Log-sigmoid function 1 f h ( x) (14) 1 e x The activation function in the output layer is the Pureline function f o ( x) x (15) The normalized failure pressure P is given by [16] N 4 h P W1oj f h W ji Ii b h bo j (16) j 1 i 1 where N is number of neurons in the hidden layer W1oj are weights in the output layer h W ji are weights in the hidden layer bo is bias in the output layer and b h are biases in the hidden layer j The output transfer function T f out ( I i ) P b / a (17)where n n a max min P max P min , i 1, 2,3, and 4 b nmin Min{au P} , i 1, 2,3, and 4
30.
19 and P is the output training pattern vector. The final failure pressure P is given by T P fout ( P) (18) Training consists of providing a set of known input-output pairs (or patterns) to thenetwork. Back-propagation learning process has two passes through the network: aforward calculation pass and an error back-propagation pass. In the forward pass, inputpatterns broadcast from input layer to output layer in order to generate the actual resultsof network. During the backward propagation, weights in each node are iterativelyadjusted based on the errors using the gradient descent equations. The procedure isrepeated until convergence is achieved. In this study, the input-output sets are obtainedfrom simulation results. The model is trained in MATLAB NNk tool box. The fasttraining Levenberg-Marquardt Algorithm is adopted in the training process.7. RESULTS AND DISCUSSION Five configurations of helical and hoop laminas shown in Table 4 are investigated inthis study. Case studies are conducted on composite cylinders with various thermalloadings and lay-up patterns. Failure pressures as a function of thickness ratio R underuniform thermal loadings for Cases 1-3 are shown in Figures 5(a-c) respectively. The rateof increase in failure pressure is higher at higher temperatures. This reflects thenonlinearity of thermal expansion coefficients with variation in temperature. For all thethree cases considered, the failure pressure increases with increase in temperature. Incomparison with Cases 2 and 3, the peak failure pressure is slightly higher than that ofCase 1. Similar results are shown in Figures 6(a-c) with gradient thermal loading. In
31.
20comparison with the uniform thermal loadings, the peak failure pressure is not evident forsome of the inner temperatures considered in figure 5(b). In those cases, all hoop laminaeare placed over helical laminae with inner temperature higher than outer temperature.Then thermal strain, arising from thermal expansion, becomes larger in all helicallaminae which cause hoop laminae to carry most of the axial loadings. Without helicallaminae sustaining major part of the axial loading, the peak pressure then disappears atlower thickness ratio area. With increasing thickness ratio, the axial-load bearing capacityof the hoop laminae increases thus resulting in the rise in failure pressure. Thisphenomenon cannot be observed in Figures 6(b-c) because the helical and hoop laminaeare laid alternatively. From Figures 6(a-c), with inner temperature increasing (from 25oCto 140oC), the failure pressure rises till it reaches the set temperature (50oC) of outsidewall, and then starts to decrease. Also it can be observed that the failure pressuredecreases as the gradient of the non-uniform temperature increases. By comparison of Cases 1, 2 and 3, the alternative lay up pattern (in Cases 2 and 3)can result in higher failure pressure than that of non-alternative lay up (in Case 1), whencylinder is experiencing uniform thermal loading and no significant increase is observedin gradient thermal loading. However, in Case 1, the location of peak pressure varies a lotin comparison with that of Cases 2 and 3 under gradient thermal loading. This largevariation might bring down the failure pressure at optimum thickness ratio whenconsidering various thermal loadings in design. There is no significant difference that canbe observed between Case 2 (constant winding angle in helical laminate) and Case 3(gradually increased winding angle in helical laminate). To study the effect of helicalwinding angle pattern on failure pressure, Cases 2, 4 and 5 ( [±20o /±89o ]6 ,
32.
21[±10o /±89o ]6 and [±30o /±89o ]6 ) are compared with different thickness ratios (R) asshown in Figure 7. For the same thickness ratio, higher peak failure pressure is observedfor smaller winding angle. Figure 8 shows the Tsai-Wu failure indicator for each helical and hoop ply in Case 2for thickness ratio, R=0.5. Curves 1 and 2 (T25-25 and T140-140 respectively) illustratethe ply failure under uniform thermal loadings while curves 3 and 4 (T25-100 and T100-25 respectively) show the failure under gradient thermal loadings (T25-25 impliesTin=25oC and Tout = 25oC). With uniform thermal loading at 140oC, the curve is observedto be flat, which implies that all the helical and hoop laminae fail simultaneously.However, at uniform thermal loading of 25oC, the helical laminae tend to fail first. Whensubjected to non-uniform thermal loading, a large slope is observed in the curves. Theinner layers fail first for T25-100 ( Tin = 25oC and Tout =100oC), while the outer layers failfor T100-25 ( Tin = 100oC and Tout =25oC). This asynchronous behavior of inner or outerlayers during failure must cause a significant drop in maximum failure pressure,assuming that the cylinder fails when any one of the laminae fails. The network is trained by using the simulation results from Cases 2, 4 and 5 shown inTable 4. There are 12 neurons used in the neural network (NNk) model and the trainingratio is set to 0.01. After the network gets converged, the model parameters are obtainedand are listed in Tables 5 and 6. The network model is then capable of predicting thefailure pressure by providing the network inputs ( R , Tin , Tout and ). To evaluate theperformance of NNk prediction, six testing cases (shown in Table 7) are studied. Thetesting data from ABAQUS simulation results, for winding angles not used before (15oand 25o), are used to compare the predicted results from the trained neural network. The
33.
22performance of the NNk is then illustrated in Figures 9(a-b), and the maximum errors arereported for each case in Table 7. It can be seen that the simulation results are in goodagreement with the results predicted by the NNk model. The trained network can,therefore, be used to predict any failure pressure within the trained ranges of temperature,winding angle and thickness ratio.8. CONCLUSIONS A doubly curved shell model accounting for transverse shear deformation is used forthermo-mechanical analysis of hydrogen composite storage cylinders. Temperaturedependent material properties of the load carrying carbon/epoxy layer and geometricnonlinearity are also considered in the numerical model. Five typical cases have beenconsidered and the analysis is carried out by applying uniform/non-uniform thermalloading and internal pressure loading. The Tsai-Wu failure criterion is employed topredict the failure pressure by checking the failure, layer by layer. Under uniform thermalloading, a temperature increase significantly increases the maximum failure pressure.Contrastively, the non-uniform thermal loading can cause an uneven load distribution andhence decrease the maximum failure pressure. The thickness ratio also plays an importantrole in determining the maximum failure pressure and should be selected appropriatelybased on the thermal and mechanical loading conditions. A neural network (NNk) modelis developed and used to predict the failure pressures. The performance of the trainedneural network is then evaluated by comparing the predicted values with those of testingcases and the results are in good agreement.
34.
23 REFERENCES[1] N. Takeichia, H. Senoha, T. Yokotab, H. Tsurutab, K. Hamadab, H. Takeshitac, H. Tanakaa, T. Kiyobayashia, T. Takanod and N. Kuriyamaa, “Hybrid Hydrogen Storage Vessel, A Novel High-pressure Hydrogen Storage Vessel Combined with Hydrogen Storage Material,” International Journal of Hydrogen Energy, Vol. 28, pp. 1121-1129, 2003.[2] C. Liang, H. Chen and C. Wang, “Optimum Design of Dome Contour for Filament- wound Composite Pressure Vessels Based on a Shape Factor,” Composite Structures, Vol. 58, pp. 469-482, 2002.[3] V. V. Vasiliev, A. A. Krikanov and A. F. Razin, “New Generation of Filament- wound Composite Pressure Vessels for Commercial Applications,” Composite Structures, Vol. 62, pp. 449-459, 2003.[4] P. Y. Tabakov and E. B. Summers, “Lay-up Optimization of Multilayered Anisotropic Cylinders Based on a 3-D Elasticity Solution,” Computers and Structures, Vol. 84, pp. 374-384, 2006.[5] J. Park, C. Hong, C. Kim and C. Kim, “Analysis of Filament Wound Composite Structures Considering the Change of Winding Angles Through the Thickness Direction,” Composite Structures, Vol. 55, pp. 63-71, 2002.[6] M. Z. Kabir, “Finite Element Analysis of Composite Pressure Vessels with a Load Sharing Metallic Liner,” Composite Structures, Vol. 49, pp. 247-255, 2000.[7] D. L. Gray and D. J. Moser “Finite Element Analysis of a Composite Overwrapped Pressure Vessel,” 40th AIAA/ASME/SAE/ASEE Joint Propulsion Conference and Exhibit, Fort Lauderdale, FL, AIAA 2004-3506, pp.1-15, July 11-14, 2004.[8] I. H. Akcay and I. Kaynak, “Analysis of Multilayered Composite Cylinders under Thermal Loading,” Journal of Reinforced Plastics and Composites, Vol. 24, pp.1169-1179, 2005.[9] O. Sayman, “Analysis of Multi-layered Composite Cylinders under Hygrothermal Loading,” Composites: Part A, Vol. 36, pp. 923-933, 2005.[10] J. M. Schneider, “Gaseous Hydrogen Station Test Apparatus: Verification of Hydrogen Dispenser Performance Utilizing Vehicle Representative Test Cylinders,” SAE World Congress & Exhibition, Detroit, MI, pp.1-10, April 2005.
35.
24[11] K. Chandrashekhara and A. Bhimaraddi, “Thermal Stress Analysis of Laminated Doubly Curved Shells using a Shear Flexible Finite Element,” Computers and Structures, Vol. 52, pp. 1023-1030, 1994.[12] K. Chandrashekhara and T. Schroeder, “Nonlinear Impact Analysis of Laminated Cylindrical and Doubly Curved Shells,” Journal of Composite Materials, Vol. 29, pp. 2160-2179, 1995.[13] F. Mitlitsky, A. H. Weisberg and B. Myers, “Vehicular Hydrogen Storage Using Lightweight Tanks,” Proceedings of the U.S. DOE Hydrogen Program Review NREL/CP-570-28890, 2000.[14] S. W. Tsai and E. M. Wu, “A General Theory of Strength for Anisotropic Materials,” Journal of Composite Materials, Vol. 5, pp. 58-80, 1971.[15] K. J. Yoon and J. Kim, “Prediction of Thermal Expansion Properties of Carbon/Epoxy Laminae for Temperature Variation,” Journal of Composite Materials, Vol.34, pp. 90-100, 2000.[16] M. T. Valoor and K. Chandrashekhara, “A Thick Composite Beam Mode for Delamination Prediction by the Use of Neural Networks,” Composite Science and Technology, Vol.60, pp. 1773-1779, 2000.
36.
25 LIST OF TABLESTable 1 Ultimate strength of carbon/epoxy compositeTable 2 Mechanical and thermal properties of S-glass/epoxyTable 3 Mechanical and thermal properties of Aluminum Alloy 6061-T6Table 4 Lay-up configurations for various winding patternsTable 5 Weights and biases for trained neural networkTable 6 Scale constants for trained neural networkTable 7 Testing cases and maximum error of prediction
37.
26 LIST OF FIGURESFigure 1 Structure scheme of hydrogen storage cylinderFigure 2 Doubly curved shell and coordinate systemFigure 3 Finite element model of hydrogen cylinderFigure 4 Feedforward back-propagation Neural Network architectureFigure 5(a) Uniform thermal loading with Tin=Tout (in Case 1)Figure 5(b) Uniform thermal loading Tin=Tout (in Case 2)Figure 5(c) Uniform thermal loading Tin=Tout (in Case 3)Figure 6(a) Gradient thermal loading with Tout=50oC (in Case 1)Figure 6(b) Gradient thermal loading with Tout=50oC (in Case 2)Figure 6(c) Gradient thermal loading with Tout=50oC (in Case 3)Figure 7 Failure pressure with inside temperature variation (Tout=25oC)Figure 8 Ply-by-ply failure predictions under various thermal loadingsFigure 9(a) Comparison of failure pressures from NNk and ABAQUS at = 15oFigure 9(b) Comparison of failure pressures from NNk and ABAQUS at = 25o
43.
32Table 6 Scale constants for trained neural network i ai bi a b 1 1.05263 -1.10526 0.05090 -1.96068 2 0.01739 -1.43478 3 0.01739 -1.43478 4 0.10000 -2.00000
44.
33Table 7 Testing cases and maximum error of prediction Testing Inputs Max. Error case Tin (oC) Tout (oC) θ (Degree) (%) 1 40 40 15 1.32 2 30 80 15 -1.54 3 130 40 15 1.23 4 40 40 25 1.11 5 30 80 25 -2.40 6 130 40 25 -1.00
45.
34 Tout Glass/Epoxy 26:-450 Glass/Epoxy 25: 450 R out Carbon/Epoxy 24: 89 0 Carbon/Epoxy 23:-890 Carbon/Epoxy 2:-100 Carbon/Epoxy 1: 100 Aluminum Tin R in PressureFigure 1 Structure scheme of hydrogen storage cylinder
46.
35Figure 2 Doubly curved shell and coordinate system
47.
36Figure 3 Finite element model of hydrogen cylinder
48.
37 b1h fh h W 11 R b2h o W11 R Tin fh bo Tin T fin o fo P f T Tout W12 out P Tout h W1o N h b N WN 4 fh Input layer Hidden layer Output layerFigure 4 Feedforward back-propagation Neural Network architecture
49.
38Figure 5(a) Uniform thermal loading with Tin=Tout (in Case 1)
50.
39Figure 5(b) Uniform thermal loading Tin=Tout (in Case 2)
51.
40Figure 5(c) Uniform thermal loading Tin=Tout (in Case 3)
52.
41Figure 6(a) Gradient thermal loading with Tout=50oC (in Case 1)
53.
42Figure 6(b) Gradient thermal loading with Tout=50oC (in Case 2)
54.
43Figure 6(c) Gradient thermal loading with Tout=50oC (in Case 3)
55.
44Figure 7 Failure pressure with inside temperature variation (Tout=25oC)
57.
46Figure 9(a) Comparison of failure pressures from NNk and ABAQUS at = 15o
58.
47Figure 9(b) Comparison of failure pressures from NNk and ABAQUS at = 25o
59.
48 PAPER II: ANALYSIS OF COMPOSITE HYDROGEN STORAGE CYLINDERS SUBJECTED TO LOCALIZED FLAME IMPINGEMENTS ABSTRACT A comprehensive non-linear finite element model is developed for predicting thebehavior of composite hydrogen storage cylinders subjected to high pressure andlocalized flame impingements. The model is formulated in an axi-symmetric coordinatesystem and incorporates various sub-models to describe the behavior of the compositecylinder under extreme thermo-mechanical loadings. A heat transfer sub-model isemployed to predict the temperature evolution of the composite cylinder wall andaccounts for heat transport due to decomposition and mass loss. A compositedecomposition sub-model described by Arrhenius’s law is implemented to predict theresidual resin content of the thermal damaged area. A sub-model for material degradationis implemented to account for the loss of mechanical properties. A progressive failuremodel is adopted to detect various types of mechanical failure. These sub-models areimplemented in ABAQUS commercial finite element code using user subroutines.Numerical results are presented for thermal damage, residual properties and the profile ofthe resin content in the cylinder. The developed model provides a useful tool for safedesign and structural assessment of high pressure composite hydrogen storage cylinders.
60.
491. INTRODUCTION High pressure composite cylinders for hydrogen storage are typically made with ahigh molecular weight polymer or aluminum liner that serves as a hydrogen gaspermeation barrier. A filament-wound, carbon/epoxy composite laminate over-wrappedon the outside of the liner provides the desired pressure load bearing capacity. Due to theflammable nature of polymer-reinforced composites, there is a high risk of failure of thecomposite hydrogen storage cylinder under accidental fire exposure. As the stiffness andstrength of composites are temperature dependent, the high pressure (usually 34.5 MPa to70.0 MPa) in the cylinder can result in catastrophic failure. Therefore, assessment ofstructural integrity of high pressure composite hydrogen storage cylinders subjected tofire exposure is necessary for safe cylinder design. Many investigations have been conducted by various researchers [1-4] on thebehavior of high pressure composite cylinders under mechanical loadings. Using finiteelement methods, numerous studies have been performed on high-pressure vesselanalysis [5-7]. Compared to pure mechanical loading and pure thermal loading, therehave been few studies on the composite cylinders subjected to the combined thermal andmechanical loads [8-9]. However, those models only consider the temperature rangebefore composite decomposition occurs and fall short of providing capability to assessthe behavior of cylinders subjected to fire impingement. To study fire effect oncomposites, different one-dimensional thermal models have been developed to predict thetemperature and the residual resin content as a function of time [10-12]. These modelsaccount for heat transfer by conduction, resin decomposition, and the cooling effect ofvolatile products passing through the laminate. Therefore, to characterize the fire
61.
50response of high pressure hydrogen composite cylinders, mechanisms of mechanicaleffect, thermal effect and decomposition have to be considered. In this paper, a coupled thermo-mechanical finite element model has been developedto simulate composite hydrogen storage cylinders subjected to high pressure and heat fluxon the wall surface. The model is formulated in an axi-symmetric coordinate systemwhich accounts for out-of-plane stresses and reduces computational cost dramatically.When the polymer materials are exposed to a sufficiently high temperature (200-300°C),decomposition reactions and thermo-chemical expansion begin to occur and the resinsystem degrades to form gaseous products and carbonaceous char. In order to incorporatethis phenomenon, the thermal model is built to account for gas convection and heatgeneration due to decomposition in addition to conduction of the composite, convectionand radiation of surface. The fire source is modeled as a constant heat flux throughout thesimulation. The inner pressure of the cylinder is dependent on the temperature ofhydrogen gas which is modeled as a sink temperature. The variation of materialproperties with temperature is significant for composites, especially at high temperatures.A temperature dependent material model has been developed and implemented. Hashin’stheory is used as a progressive failure criterion to predict different types of failure (matrixcracking and fiber breakage). These models are developed and implemented in acommercial finite element code ABAQUS, using user subroutines. A typical highpressure hydrogen composite cylinder is simulated using the developed model and resultsfrom the parametric study are reported.
62.
512. MODELING OF HIGH PRESSURE COMPOSITE HYDROGEN STORAGECYLINDERS A strong sequentially coupled thermal-stress analysis approach is implemented forpredicting the behavior of composite hydrogen cylinders subjected to flameimpingements and high internal pressure. At each increment, the temperature profile isobtained using the thermal and resin reaction models. The temperature field is thenimported to the mechanical model with material damage information from the previousincrement. The pressure of the inner cylinder is updated based on the heat absorption ofhydrogen gas, which is computed from the temperature profile. The thermal andmechanical models are solved sequentially in each increment. As the wall consists of alarge number of laminae, modeling each lamina will cause extraordinary computationalcost, especially when thermal and damage models are also incorporated. Hence, ahomogenization technique is used to smear several laminae to a sub-laminate as in Figure1. The equivalent moduli of the sub-laminate are used in the formulation of the finiteelement model.2.1 Thermal Model The high temperature will cause resin decomposition of the cylinder composite wall.The decomposition rate of the resin is usually represented by Arrhenius’s law and can beexpressed as [13]: A exp( EA / RT ) (1) twhere, – density
63.
52 t – time T – temperature A – pre-exponential factor E A – activation energy R – gas constant Material constants A and EA are determined using Differential Scanning Calorimetry.In consideration of the resin reaction, the heat transfer equilibrium equation has toinclude resin decomposition energy and vaporous migration energy. Since the dimensionin the thickness direction is much less than that of hoop and axial directions, the vaporousgas is only assumed to transfer in thickness direction. The axi-symmetric heat diffusionequation can be written as [14]: T T 1 T T T C p kr kr kz mg C pg t r r r r z z r t Q hcom hg (2)where, C p – specific heat of the composite k – thermal conductivity r – displacement through the thickness mg – gas mass flux C pg – specific heat of the gas Q – heat of decomposition hcom – enthalpy of the composite hg – enthalpy of hydrogen gas
64.
53 The mass flow direction of the gas generated in the laminate is towards the hot face ofthe laminate. The total mass flux of the generated gas at a specific spatial location in thelaminate is the sum of the gas mass flux generated from the inner face to this spatiallocation. The gas mass flux at any spatial location can be calculated as: rh mg drh (3) tW t where, rh – distance from the hot face tW – wall thickness of the composite2.2 Sub-laminate Model The principle of sub-laminate (Figure 1) homogenization is based on the assumptionthat the in-plane strains and the interlaminar stresses through the thickness are constant[15-18]. The lamina stress-strain relationship in a global coordinate can be written as: o Coo Coi o (4) i Coi Cii i where, Coo , Coi and Cii are sub matrices of global stiffness matrix, Coi is the transpose ofCoi , o and i are out-of-plane and in-plane stresses respectively, o and i are out-of-plane and in-plane strains respectively. represents the term is constant through thelaminate. Partially inverting Eq. (4) yields: o Coo1 Coo1Coi o (5) 1 i Coi Coo 1 Coi Coo Coi Cii i After averaging, Eq. (5) can be expressed as:
65.
54 o A B o T (6) i B D i N N N t k 1where, A t Coo , B ttk Coo1Coi , D ttk CoiCoo1Coi Cii k 1 k k 1 k k 1 ktk is the thickness of each lamina in the smeared sub-laminate and t is the total thicknessof the smeared sub-laminate. Partially inverting Eq. (6) yields the equivalent stiffness matrix Qeq of the sub-laminate as: o A 1 A 1 B o T 1 T 1 (7) i B A B A B D i The equivalent compliance matrix is given by: 1 1 A1 A1B [Qeq ] T 1 [Sij ] (8) B A BT A1B D Equivalent engineering properties used for the simulation can be obtained from Eq.(8) as: E11 1/ S44 , E22 1/ S55 , E33 1/ S11 G12 1/ S 66 , G13 1/ S33 , G23 1/ S22 (9) v12 S45 / S44 , v13 S14 / S 44 , v23 S15 / S55 After the global stresses and strains of the sub-laminates are obtained, the stresses ineach lamina are obtained in the global material coordinates as: o k o (10) i k BT k o D k i where k is the k th lamina of the sub-laminate.
66.
55 Finally, the stresses in the local material coordinate system can be obtained bystandard coordinate transformation.2.3 Formulation of Finite Element Model Axi-symmetric formulation for transient analysis can be written as: [M e ]{ e } [ K e ]{e } {F e } {FTe } (11)where [M e ] 2 [ N ]T [ N ]rdS , [ K e ] 2 [ B]T [C ][ B]rdS , { e } {{ur } {u } {uz } }T , s s{F e } and {FTe } are forces due to mechanical and thermal loads respectively. In addition,N is an interpolation function, B is the strain displacement function, C is the elasticitymatrix, is the density, and ur , u , u z are displacement components in the cylindricalcoordinate system. By discretizing Eq. (2), the heat conduction formulation can be expressed as [CT ]{T } [ KT ]{T } {HT } (12)where[CT ] C p N T NdV , [ KT ] N T k N dV , [ H T ] N T qs dS N T qr dV . V V S Vwhere k is thermal conductivity, qs is surface heat flux and qr is the reaction heat due toresin decomposition and vaporous migration. The reaction heat qr can be expressed as T qr mg C pg Q (C pg C p ) (T T ) (13) r t where, C pg is the specific heat of gas, T is ambient temperature and Q is the heat ofdecomposition.
67.
56 Combining Eq. (11) and (12), the sequentially coupled thermal-stress equation can bewritten as: e e 0 0 e K e e e e M 0 0 F FT (14) 0 0 0 0 CT T 0 KT T {H T } 3. MATERIAL MODELS3.1 Temperature Dependent Material Properties Mechanical and thermal properties of fiber reinforced composites vary significantlywith temperature. As the carbon/epoxy laminate carries the pressure loading from thehydrogen gas, the effect of temperature on its material properties cannot be ignored.However, a complete set of temperature dependent properties is not available in theliterature. Assumptions and curve fittings are necessary to obtain the material propertydata based on the limited experimental data that is available. Numerous studies have beendone on curve fitting of temperature dependent properties. Gibson et al. [19] shows that ahyperbolic tan (tanh) function is capable of giving an excellent fit to experimental datafor material moduli and strength. The equation can be expressed as: P PR P PR P(T ) U 2 U 2 tanh k T Tg C (15)where, P(T ) is the temperature dependent material property, P is the unrelaxed (low Utemperature) value of that property, PR is the relaxed (high temperature) value of thatproperty, k is a constant describing the width of the distribution, T is temperature, Tg is themechanically determined glass transition temperature and C is a constant.
68.
57 Experimental data for carbon/epoxy composite are taken from the literature [20-22].Moduli are fitted using Eq. (15). The curve fitting parameters are listed in Table 1. Thethermal properties of carbon/epoxy are listed in Table 2 and Table 3. Properties for theresin reaction model are listed in Table 4. The strength of the composite is dependent on temperature and resin content. It hasbeen assumed that the temperature variation of the ultimate longitudinal, transverse andshear strengths of carbon/epoxy follow the same pattern as the longitudinal, transverseand shear moduli respectively and resin content only affects the transverse and shearstrengths. The virgin strengths used this investigation are listed in Table 5.3.2 Composite Failure Criteria As the composite wall of the hydrogen cylinder experiences combined mechanicaland thermal loads, a variety of failure types would occur in the process. A progressivefailure model is employed in this study to identify the failure types based on failurecriterion and predict the safety state of the cylinder. Hashin’s failure criterion [23],accounting for four possible modes of ply failure, is used for this purpose.1. Matrix tensile or shear cracking ( 22 33 0 ) 2 I mt 33 22 2 2 2 12 13 23 22 33 (16) t 2 S 2 F T F LT2. Matrix compressive or shear cracking ( 22 33 0 ) 2 2 1 FTc 22 33 12 13 23 22 33 2 2 2 I mc c 1 (17) 2 FLT S 22 33 S 2 4 FLT S 2 FT FLT 3. Fiber tensile fracture ( 11 0 )
69.
58 2 1 I ft 11 t S 2 12 13 2 2 (18) FL FLT 4. Fiber compressive fracture ( 11 0 ) I fc 11 c (19) FL where, FLt , FLc , FTt , FTc and FLT are longitudinal tensile strength, longitudinal compressive Sstrength, transverse tensile strength, transverse compressive strength and shear strength ofunidirectional ply respectively. Once a specific type of failure is identified in the laminate, the reduction in its load-carrying capacity is accounted for, by a reduction in its elastic moduli based on Tansassumption [24]: (a) When matrix tensile or shear cracking occurs, properties( E22 , G12 , G23 ) are taken as 0.2 times the original values. (b) When matrixcompressive or shear cracking occurs, properties ( E22 , G12 , G23 ) are taken as 0.4 timesthe original values. (c) When fiber tensile fracture occurs, E11 is taken as 0.07 times theoriginal values. (d) When fiber compressive fracture occurs, E11 is taken as 0.14 timesthe original values.3.3 Model for Hydrogen Gas The hydrogen gas in the cylinder absorbs energy and increases the internal pressure.In the present study, the hydrogen gas effect is modeled as a sink whose temperature isupdated at each increment based on the amount of heat flux going through the innercylinder surface. The internal pressure of the cylinder is computed from the state equationof hydrogen. Experimental data for hydrogen gas is taken from the literature [25]. The
70.
59pressure and temperature relationship at a constant density of 23.59 kg/m3 (when thetemperature is 20°C and the pressure is 34.5 MPa) is curve fitted as shown in Figure 2.The fitted equation is employed to compute cylinder internal pressure.4. FINITE ELEMENT SIMULATION PROCEDURE The cylinder dimensions used in the present study are based on the design proposedby Mitlitsky et al. [26] and are summarized in Table 6. An axi-symmetric finite elementmodel is built in ABAQUS as shown in Figure 3. The length of the cylindrical part istaken as Lc 0.3 for analysis and the dome curve follows a geodesic path. The flamesource is modeled as a constant heat flux (75 kW/m2) applied on the area with length Lsthroughout the analysis. The radiation, as well as the convection, is also considered at thecylinder outside surface. Pressure is imposed on the inner liner surface. A symmetricboundary condition is applied at the end of the cylinder to reduce the model to half of thecylinder. The model uses SAX8RT element accounting for both deformation and heattransfer. The cylinder wall consists of a inner aluminum liner and six sub-laminates ofcarbon/epoxy (Figure 4). Each hoop (90) and helical (±10) sub-laminate consists ofmany laminas. The implementation procedure of the developed models in ABAQUS is summarizedas shown in Figure 5 and the names of interface subroutines are listed in parentheses. Ateach increment, the material properties are updated (using subroutine USDFLD) based onthe information of current temperature, failure type and resin content. The mechanicalloading vector is computed from the hydrogen gas model (in the subroutine FILM). The
71.
60hydrogen gas model provides the sink temperature from which the internal pressure ofthe cylinder is computed (from subroutine DLOAD) using the gas state equation. Forthermal loading vector, the flame source, resin decomposition, and mass flux of burninggas contribute the heat flux collaboratively (calculated in subroutine HETVAL). Thecoupled thermo-mechanical equations are then solved to get the global stresses andtemperature field. The lamina stresses are retrieved from global stresses and importedinto the failure model to compute failure indices. At the next increment, all sub-models(resin sub-model, hydrogen gas sub-model and material strength sub-model) are solvedbased on the temperature field and failure type from the previous increment. Theprocedure iterates until the specified time is met. In the present study, this transientanalysis is carried out for 1000 seconds.5. RESULTS AND DISCUSSION The heat exchange rate between the hydrogen gas and aluminum liner affects theincrease in sink temperature (temperature of hydrogen gas) when the cylinder is subjectedto flame impingement. In the simulation, the heat exchange rate is represented by a filmcoefficient (H). A parametric study is conducted on H ranging from 10 to 10,000W/m2/°C. The results are shown in Figure 6. The sink temperature increases rapidly withH at the beginning and flattens out at higher values of H. At higher H values, the sinktemperature is not sensitive to the heat exchange rate. In real situations, this value canvary over a large range with variation of hydrogen flow rate. H is taken as 1000 W/m2/°Cfor convenience throughout the analysis. Figure 7 plots the internal pressure variationwith time for different flame impingement sizes. The non-dimensional L is defined as
72.
61L=Ls/Lc (Figure 3). It can be seen that at the beginning the internal pressure increasesvery slowly and is much higher after 200 seconds. With increasing size of the flame area,the pressure goes up. For the rest of analysis, results are reported at L = 0.1. Figure 8 shows the temperature distributions of the liner internal surface at differenttimes. The temperature of flame impingement center is higher than the adjacent areas.Figure 9 shows the temperature distributions of the composite through the thicknessdirection at the flame center. The temperature of the outermost sub-laminate 6 increasesto 520°C in the first 200 seconds and then continues to go up very slowly during the restof the time. The innermost sub-laminate 1 increases slowly during the entire flameimpingement process. Figure 10 shows the residual resin content in the compositethrough the thickness at the flame center. In the outermost sub-laminate 6, resin isdepleted totally in the first 100 seconds and in the innermost sub-laminate 1, the resincontent keeps almost constant throughout the entire process. Stress distributions through the composite thickness at the end of the simulation timeare reported in Figures 11 and 12. An uneven stress (S11) distribution is observed in thefiber direction for hoop sub-laminates. This can result in the breakage of fibers in theinner hoop layers. The stresses in the transverse direction (S22) and thickness direction(S33) are plotted in Figure 12. The shear stresses are not reported as they are negligiblysmall. Failures due to fiber fracture, matrix cracking and resin depletion are presented inFigure 13 (a-c). A higher fiber fracture index is observed for the inner layer. This isbecause the fibers of outer layers cannot bear much mechanical load as the resin is eitherdepleted or softened due to the high temperature. Matrix cracking is observed at the inner
73.
62half of the composite wall. However, the matrix failure index is very low at the outermostlayers, since there is not much matrix (resin) left. Hence, no significant mechanicalloading can be carried in this part. This can be observed in Figure 13(c).6. CONCLUSIONS A comprehensive finite element model has been developed to analyze compositehydrogen storage cylinders subjected to high pressure and flame impingements. Themodel considers the resin reaction, heat exchange between the hydrogen gas and liner,and the progressive failure process. A sub-laminate model has been developed to reducethe computational time. A temperature dependent material model and the failure modelshave been developed and implemented to accurately predict various types of failure forthe hydrogen storage cylinder. All the models are formulated in an axi-symmetriccoordinate system and implemented in ABAQUS through user subroutines. Analysis of atypical high pressure composite hydrogen cylinder under fire exposure is conducted byusing the developed model. Parametric studies are done on heat exchange rate (betweenhydrogen gas and liner) and the size of flame source. Stresses, temperature profile andfailure types are reported. The developed model can be used to accommodate varioustypes of thermal and mechanical loadings, lamina stacking sequence, and laminathickness to establish safe working conditions and design limits for hydrogen storagecylinders. In addition, this simulation process can be used for both type III and type IVhydrogen cylinders, as both have a similar structure except for the type of liner beingused.
74.
63 REFERENCES[1] C. Liang, H. Chen and C. Wang, “Optimum Design of Dome Contour for Filament- wound Composite Pressure Vessels Based on a Shape Factor,” Composite Structures, Vol. 58, pp. 469-482, 2002.[2] V. V. Vasiliev, A. A. Krikanov and A. F. Razin, “New Generation of Filament- wound Composite Pressure Vessels for Commercial Applications,” Composite Structures, Vol. 62, pp. 449-459, 2003.[3] P. Y. Tabakov and E. B. Summers, “Lay-up Optimization of Multilayered Anisotropic Cylinders Based on a 3-D Elasticity Solution,” Computers and Structures, Vol. 84, pp. 374-384, 2006.[4] D. Chapelle and D. Perreux, “Optimal Design of a Type 3 Hydrogen Vessel: Part I- Analytic Modeling of the Cylindrical Section,” International Journal of Hydrogen Energy, Vol.31, pp. 627–638, 2006.[5] J. Park, C. Hong and C. Kim, “Analysis of Filament Wound Composite Structures Considering the Change of Winding Angles through the Thickness Direction,” Composite Structures, Vol. 55, pp. 63-71, 2002.[6] M. Z. Kabir, “Finite Element Analysis of Composite Pressure Vessels with a Load Sharing Metallic Liner,” Composite Structures, Vol. 49, pp. 247-255, 2000.[7] D. L. Gray and D. J. Moser “Finite Element Analysis of a Composite Overwrapped Pressure Vessel,” 40th AIAA/ASME/SAE/ASEE Joint Propulsion Conference and Exhibit, Fort Lauderdale, FL, AIAA 2004-3506, pp. 1-15, July 11-14, 2004.[8] I. H. Akcay and I. Kaynak, “Analysis of Multilayered Composite Cylinders under Thermal Loading,” Journal of Reinforced Plastics and Composites, Vol. 24, pp. 1169-1179, 2005.[9] O. Sayman, “Analysis of Multi-layered Composite Cylinders under Hygrothermal Loading,” Composites: Part A, Vol. 36, pp. 923-933, 2005.[10] J. B. Henderson, J. A. Wiebelt and M. R. Tant, “A Model for the Thermal Response of Polymer Composite Materials with Experimental Verification,” Journal of Composite Materials, Vol. 19, pp. 579-595, 1985.[11] J. B. Henderson and T. E. Wiecek, “A Mathematical Model to Predict the Thermal Response of Decomposing, Expanding Polymer Composites,” Journal of Composite Materials, Vol. 21, pp. 373-393, 1987.[12] A. G. Gibson, P. N. H. Wright and Y-S. Wu, “The Integrity of Polymer Composites during and after Fire,” Journal of Composite Materials, Vol. 38, pp. 1283-1307, 2004.[13] K. J. Laidler, “Theories of Chemical Reactions Rates,” McGraw-Hill: New York, 1969.[14] J. Lua, J. OBrien, C. T. Key, Y. Wu and B. Y. Lattimer, “A Temperature and Mass Dependent Thermal Model for Fire Response Prediction of Marine Composites,”
75.
64 Composites Part A: Applied Science and Manufacturing, Vol. 37, pp.1024-1039, 2006.[15] P. C. Chou and J. Carleone, “Elastic Constants of Layered Media,” Journal of Composite Materials, Vol. 6, pp. 80-93, 1972.[16] C. T. Sun and S. Li, “Three-dimensional Effective Elastic Constants for Thick Laminates,” Journal of Composite Materials, Vol. 22, pp. 629-639, 1988.[17] H. Chen and S. W. Tsai, “Three-dimensional Effective Moduli of Symmetric Laminates,” Journal of Composite Materials, Vol. 30, pp. 906-916, 1996.[18] J. Whitcomb and J. Noh, “Concise Derivation of Formulas for 3D Sublaminate Homogenization,” Journal of Composite Materials, Vol. 34, pp. 522-535, 2000.[19] A. G. Gibson, Y.-S. Wu, J. T. Evans and A. P. Mouritz, “Laminate Theory Analysis of Composites under Load in Fire,” Journal of Composite Materials, Vol. 40, pp. 639-658, 2006.[20] K. J. Yoon and J. Kim, “Prediction of Thermal Expansion Properties of Carbon/Epoxy Laminates for Temperature Variation,” Journal of Composite Materials, Vol. 34, pp. 90-100, 2000.[21] G. Kalogiannakis, D. V. Hemelrijck and G. V. Assche, “Measurements of Thermal Properties of Carbon/Epoxy and Glass/Epoxy using Modulated Temperature Differential Scanning Calorimetry,” Journal of Composite Materials, Vol. 38, pp. 163-175, 2004.[22] G. Liang, A. Garg, K. Chandrashekhara, V. Flanigan and S. Kapila, “Cure Characterization of Pultruded Soy-based Composites,” Journal of Reinforced Plastics and Composites , Vol. 24, pp. 1509-1520, 2005.[23] Z. Hashin, “Failure Criteria for Unidirectional Fiber Composites,” Journal of Applied Mechanics, Vol. 47, pp. 329-334, 1980.[24] S. C. Tan, “A Progressive Failure Model for Composite Laminates Containing Openings,” Journal Composite Materials, Vol. 25, pp. 556-577, 1991.[25] W. E. Deming and L. E. Shupe, “Some Physical Properties of Compressed Gases, III. Hydrogen,” Physical Review, Vol. 40, pp. 848-859, 1932.[26] F. Mitlitsky, A. H. Weisberg, and B. Myers, “Vehicular Hydrogen Storage using Lightweight Tanks,” Proceedings of the 2000 U.S.DOE Hydrogen Program Review, NREL/CP-570-28890, pp. 1-82, 2000.
76.
65 LIST OF TABLESTable 1 Curve fitting parameters for transverse and shear modulusTable 2 Thermal expansion coefficients of carbon/epoxyTable 3 Specific heat and thermal conductivity of carbon/epoxyTable 4 Parameters for resin reaction modelTable 5 Strength of carbon/epoxyTable 6 Design parameters for the cylinder
77.
66 LIST OF FIGURESFigure 1 Schematic of hydrogen cylinderFigure 2 Curve fitting for hydrogen gas state equation at constant densityFigure 3 Finite element model of the cylinderFigure 4 Stacking sequence of the cylinder wallFigure 5 Finite element implementation schemesFigure 6 Variation of sink temperature with film coefficientFigure 7 Internal pressure variation with time for various flame area sizesFigure 8 Temperature distributions along the length at inner surface of the aluminum linerFigure 9 Temperature distributions through composite thicknessFigure 10 Residual resin content through the thicknessFigure 11 Stress (S11) distribution through the thicknessFigure 12 Stress (S22, S33) distribution through the thicknessFigure 13(a) Fiber fracture index (Imt) contour around heat sourceFigure 13(b) Matrix cracking index (Ift) contour around heat sourceFigure 13(c) Density index (ρ/ρ0) contour around heat source
78.
67Table 1 Curve fitting parameters for transverse and shear modulus Longitudinal Transverse Shear modulus modulus modulus PU(GPa) 133.35 9.135 4.515 PR(GPa) 111 0.1 0.045 K 0.0064 0.022 0.02 C 1 1 1 Tg (oC) 100 100 100
85.
74 1000 Fitting curve 900 Test data 800 Equation: P = 1.2 T + 320 Pressure (Bar) 700 600 500 400 300 0 100 200 300 400 500 o Temperature ( C)Figure 2 Curve fitting for hydrogen gas state equation at constant density
86.
75 Flame source Ls Symmetric boundary Lc Hydrogen gasCentral axis of axisymmetirc modelFigure 3 Finite element model of the cylinder
87.
76 Flame source o Hoop Sublaminate 6 (90 )Helical Sublaminate 5 ( 10 o ) Hoop Sublaminate 4 (90 o ) Carbon/epoxyHelical Sublaminate 3 ( 10 ) o composite Hoop Sublaminate 2 (90 o )Helical Sublaminate1 ( 10 o ) Aluminum Liner Inner pressure Figure 4 Stacking sequence of the cylinder wall
88.
77Figure 5 Finite element implementation schemes
89.
78 120 100Temprature (oC) 80 60 40 20 0 2000 4000 6000 8000 10000 2o H (W/m / C) Figure 6 Variation of sink temperature with film coefficient
90.
79 60 55 Pressure (MPa) 50 L=1.0 L=0.5 45 40 L=0.1 35 30 0 200 400 600 800 1000 Time (Sec)Figure 7 Internal pressure variation with time for various flame area sizes
91.
80 120 100 Time = 1000 Sec Temperature (oC) Time = 800 Sec 80 Time = 600 Sec 60 Time = 400 Sec 40 Time = 200 Sec 20 Time = 0 Sec 0 0 2.5 5 7.5 10 12.5 15 Distance from flame center (cm)Figure 8 Temperature distributions along the length at inner surface of the aluminum liner
95.
84 5 0 S 22 -5(MPa) -10 33S -15 22S S33 -20 -25 -30 0 2 4 6 8 10 12 Distance (mm) Figure 12 Stress (S22, S33) distribution through the thickness
96.
85Figure 13(a) Fiber fracture index (Imt) contour around heat source
97.
86Figure 13(b) Matrix cracking index (Ift) contour around heat source
98.
87Figure 13(c) Density index (ρ/ρ0) contour around heat source
99.
88 PAPER III: FRACTURE ANALYSIS OF HYDROGEN STORAGE COMPOSITE CYLINDERS WITH LINER CRACK ACCOUNTING FOR AUTOFRETTAGE EFFECT ABSTRACT An understanding of fracture behavior is crucial to the safe installation and operationof high pressure composite cylinders for hydrogen storage. This work has developed acomprehensive finite element model to investigate axial surface flaws in cylinder linersusing the fracture mechanics and a global-local finite element technique. Since theautofrettage process has a strong influence on cylinder fracture behavior, it is alsoconsidered in this analysis. The simulation process is broken down into three steps inorder to precisely extract fracture parameters and incorporate the autofrettage effect. Inthe first step, the global model performs the autofrettage simulation to study the residualstress with consideration of both material hardening and the Bauschinger effect. In thesecond step, the global model uses residual stress to compute displacement for the localmodel. Finally, in the third step, the local model extracts the values of stress intensityfactor (K) and J-integral. Comparison is conducted on the fracture parameters withvarious autofrettage levels and crack shapes. The vicinity of crack front is also studied bythe size and shape of the plastic zone, and the validity of stress intensity factor (K) and J-integral dominances is examined.
100.
891. INTRODUCTION High pressure composite cylinders have gained the intensive attention of theautomotive industry as hydrogen storage media for hydrogen vehicles [1]. Thesecylinders are typically made of an aluminum liner wrapped with carbon/epoxycomposites. The composite wrap is designed to withstand high pressure loading (5,000-10,000Psi) of compressed hydrogen gas while maintaining a light weight through the useof high strength, low density composite materials. The aluminum liner serves as thehydrogen barrier layer since the material provides a perfect resistance for hydrogenpermeation [2]. However, this advantage is undermined by manufacturing defects thatlead to the development of cracks in the liner. Due to the driving force from the internalpressure, continuous propagation of cracks will lead to serious leakage and eventualfailure of the cylinder. The fracture behavior of the aluminum liner, therefore, is a keyfactor affecting the operational safety and design life expectancy of the cylinder. Fracture analysis of composite cylinders stems from studies of various pipes andvessels. Since surface flaws commonly occur in these products and propagate duringservice, they are involved in most studies. In general, surface flaws are represented in theanalysis by semi-elliptical shapes. Fracture parameters such as the stress intensity factor(K) and the J-integral, which determine the crack criteria and cause of failure, arecomputed along the front of a semi-elliptical crack [3,4]. Due to their geometriccomplexity, only a few analytical solutions have been proposed to determine thoseparameters with low computational cost [5-7]. Since those methods rely on simplifiedassumptions about material models and the stress field near the crack tip, they aresuitable for a simple geometry and linear analysis.
101.
90 The finite element (FE) method provides a more general and flexible tool forevaluation of both stress intensity factor (K) and J-integral, and results have been widelyreported in the literature. Rice and Levy [8] introduced a line-spring element model tocompute K, and that work was expanded by Lee and Parks [9] to evaluation of J-integraland T stress. Raju et al. [10] computed K for internal and external surface cracks incylindrical vessels using a 3D continuum element. Kim et al. [11] analyzed internal axialsurface cracks in cylinders considering various geometric ratios and material plasticity.Diamantoudis and Labeas [12] modeled the cracks at various locations on a pressurevessel using a global-local FE technique. Guerrero et al. [13] improved a pressure vesseldesign based on a detailed FE fracture analysis. Su et al. [14-16] performed fractureanalysis on a series of compressed natural gas cylinders. Based on previous studies, mostresearch has addressed to metallic cylinders, and few studies have focused on metallicliners with a composite wrap in the hoop direction. Still less work has studied the fullcomposite-wrapped cylinder with consideration of the autofrettage effect. Autofrettage is a metal fabrication technique, commonly used in increasing durabilityof high-pressure cylinders, cannon barrels and diesel engines. In this technique, thecylindrical product is subjected to enormous pressure, causing internal portions of thepart to yield and resulting in internal compressive residual stresses to enhance productfracture performance. Since autofrettage has strong influence on cylinder fracturebehavior, this paper investigates liner cracks of high pressure composite cylinders forhydrogen storage considering autofrettage effect using fracture mechanics and a global-local FE technique. The global-local FE model has been developed in a commercial FEcode, ABAQUS. The autofrettage effect is studied in the global model. The local model,
102.
91which is driven by the results of the global model, analyzes the crack in detail to ensureaccurate computation of fracture parameters. Results for both K and the J-integral arereported for four autofrettage levels along the crack front. The effect of crack size is alsoexamined using cracks with various depth/thickness and depth/width ratios. In addition,since the stress field in the vicinity of the crack tip determines the validity of fractureparameter characterization, which is crucial for design parameter selection, the plasticzone around the crack front is studied.2. METHODOLOGY A schematic of a hydrogen composite cylinder with an inner surface flaw is shown inFigure 1. The inner liner is made of aluminum alloy that serves as a hydrogen gaspermeation barrier. Filament-wound carbon/epoxy composite laminates wrap the liner inboth the hoop and the helical directions. These laminates provide the desired pressureload bearing capacity. Due to the inner hydrogen pressure, cracks develop as a result ofmanufacturing defects and propagate in the liner wall during service. In order to restraincrack propagation, the autofrettage process is conducted before the cylinder enters serviceby introducing proper compressive stresses in the liner [17]. Stress intensity factor (K)and the J-integral provide a means to study the fracture performance of the cylinderaccording to the various deformation states.2.1 The Autofrettage Effect on Hydrogen Storage Composite Cylinders The fracture resistance of composite hydrogen cylinders can be improved by theautofrettage process, in which the cylinder is pressurized to a specified proof pressure toproduce a desired compressive stress level in the liner. Figure 2 illustrates the process
103.
92with stress-strain and load versus time curves. The autofrettage process is conducted inthe first cycle pressure loading (0→2→4) as shown in Figure 2(b). Afterwards, thepressure will cyclically remain between zero and operating pressure ( 4 ↔ 4 ) in service. During autofrettage (0→2), the composite wrap responds linearly in an elastic state,as represented by the dotted line from 0 to A in Figure 2(a). At the same time, the linerundergoes elasto-plastic deformation represented by the solid curve (0→1→2). Largeplastic deformation is introduced in the liner when the cylinder is overstressed to theproof pressure level. In the unloading process (2→4), the cylinder pressure returns to 0.The composite wrap goes from A to C, where it remains in tension. It compresses theliner linearly from point 2 to point 3 and plastically to point 4. At this point, the balancebetween the composite wrap and the liner is established, and the compressive stress c isintroduced into the liner. During service ( 4 ↔ 4 ), the aluminum liner operates in( 4 ↔ 4 ), and the composite wrap remains in (C↔B). The fracture analysis conductedhere focuses on the service stage. The selection of a proof pressure is crucial for the success of the autofrettage process.The following factors are considered in the process: (a) composite wrap strength, (b) linermaterial yielding strength, (c) Bauschinger effect, and (d) liner buckling. A maximumproof pressure selected should be smaller than the maximum pressure sustainable by thecomposite wrap, with a safety margin in case of damage to the composite. There isanother trade-off for the selection of yielding strength of liner materials. The hysteresisloop is to be formed as the yielding strength is too low while not much compressive stresscan be introduced if it is too high. In addition, the compressive yielding strength c isaffected by the Bauschinger effect which implies extremely high proof pressure may not
104.
93introduce high compressive stress in the liner. Furthermore, the compressive pressureintroduced must not exceed the critical buckling stress of the liner wall, which can beexpressed as [18]: E t crit (1) 3(1 v 2 ) R where E is Young’s modulus, v is Poisson’s ratio, t is the wall thickness of the liner, andR is the cylinder radius.2.2 Stress Intensity Factor (K) Evaluation Since very few practical problems have closed-form stress intensity factor (K)solutions, numerical methods are widely used as an alternative for problems withcomplex geometric configurations and loadings. The approaches implemented innumerical evaluation generally fall into two categories: point matching and energymethods [19]. Point matching method derives from the formula of stress anddisplacement fields near the crack tip, but it requires a high degree of mesh refinementfor reasonable accuracy. Earlier energy methods, such as J contour integration, elementalcrack advance, and virtual crack extension, compute K based on the energy release rate inthe body; however, separation of mixed-mode K components is difficult with thesemethods. An interaction integral method is used in ABAQUS to extract the individual stressintensity factor (K) for a crack from the domain integral procedure [20-21]. This methodis more accurate and efficient than earlier energy methods, and it is applicable to bothisotropic and anisotropic linear materials under monotonic loading. The expression of Kcan be written as:
105.
94 K 4 B J int (2) where K is the K vector and J int is the interaction integral vector, both with threecomponents according to three modes, and B is a pre-logarithmic energy factor matrix.For homogeneous, isotropic materials, B is given by: 8 (1 2 ) / E 0 0 2 B 0 8 (1 ) / E 0 (3) 0 0 4 / G where E is Young’s modulus, v is Poisson’s ratio, and G is the shear modulus. The interaction integral vector J int is evaluated by the domain integral procedure andcan be expressed as: J int lim n M q d (4) with M given by: u u M : aux I aux (5) x aux xwhere is equal to I, II, and III according to the three modes of fracture mechanics, is the contour that encloses the crack tip, n is the outward normal of , q is the crack extension direction, u is the displacement vector, x is the coordinate vector, I is the identity matrix, and , aux and aux are stress, auxiliary stress, and strain respectively.2.3 J-Integral Evaluation The energy domain integral method is formulated in [22] to provide a generalframework for numerical analysis of the J-integral. This method has been adopted byABAQUS for its easier numerical implementation and higher accuracy with coarser meshcompared with earlier energy methods. In the domain integral technique, a closed contour
106.
95( C C C ) is constructed around the crack as illustrated in Figure 3. The innercontour is vanishingly small, while the outer contour C is finite. Using the divergencetheorem, the 2D quasi-static contour integral is converted to domain integral on closedarea A , which is defined by: u J H q d t q d (6) A x C C xwith tensor H given by: u H WI (7) x where t is the surface traction force, q is equal to q on and vanishes on C , and W isthe strain energy. For elasto-plastic material, plastic dissipation is also included in W ,which implies that the J-integral calculation of this condition is applicable only formonotonic loading. The 3D domain integral can be obtained by expanding a 2D contouralong crack front S for a virtual distance dS to form an integral on volume V . The ABAQUS software defines the domain in terms of rings of elements surroundingthe crack tip [21]. The first contour consists of those elements directly connected tocrack-tip nodes. The second contour includes the elements in the first contour and thenext ring of elements that share nodes with the elements in the first contour. Eachsubsequent contour is defined by adding the next ring of elements that share nodes withthe elements in the previous contour.2.4 Material Models Several material models are used in the simulation to describe the behavior of thecylinder wall. The composite wrap is formulated by doubly curved laminated shell theorywith an orthotropic material constitutive model given by:
107.
96 11 1/ E1 12 / E1 13 / E1 0 0 0 11 22 12 / E1 1/ E2 23 / E2 0 0 0 22 33 13 / E1 23 / E2 1/ E3 0 0 0 33 0 0 0 1/ G12 0 0 12 (8) 12 0 0 0 0 1/ G13 0 13 13 0 0 0 0 0 1/ G23 23 23 where Ei is Young’s moduli, Gij is the shear moduli, and ij is Poisson’s ratios. To simulate the autofrettage process, an elasto-plastic material model is used tocapture deformation of the aluminum liner in the global model. The nonlinearisotropic/kinematic hardening law is employed to account for the Bauschinger effect. Theyield surface is governed by the Mises flow rule: f y 0 (9)with equivalent Mises stress given by: 3 f 2 S dev : S dev (10)where is the back stress, dev is the back stress deviator, and S is the stress deviator. The hardening law is given by: 1 C pl pl (11) y where is the back stress rate, pl is the equivalent plastic strain rate, C is the kinematicmodulus, and is the slip rate. C and are calibrated by material test data. In the submodel, different elastic models are implemented for the aluminum lineraccording to computational requirement of fracture parameters. To extract K along thecrack front, linear elastic material model is required by the interaction integral method.Instead of using an elasto-plastic model, Ramberg-Osgood (R-O) nonlinear elastic modelis used in J-integral evaluation, thus eliminating the loading effect on the accuracy of
108.
97domain integration. The one-dimension expression of the R-O model can be expressedas: n (12) 0 0 0 where is a dimensionless constant and n is the strain hardening exponent. The modelis directly related to the description of the singularity field around the crack tip and it iswidely used for curve-fitting the stress-strain data. The 3D format, used in the simulation,can be expanded from Eq.(12) as: n 1 3 q E 1 S 1 2 pI S (13) 2 0 where E is Young’s modulus, is Poisson’s ratio, p is the equivalent hydrostatic stress,q is the von-Mises equivalent stress, and S is the stress deviator. Distinction between the K dominance and J-integral dominance is characterized bythe size of the plastic zone in the vicinity of the crack tip. The radius of a critical plasticzone is given by: 2 1 K rp IC (14) 6 y where K IC is the mode I fracture toughness and y is the yielding strength. The domainof the plastic zone is obtained by identifying the region where the asymptotic stress aheadof the crack tip equals the yielding stress.
109.
983. FINITE ELEMENT SIMULATION The semi-elliptical crack is required to be modeled in substantial detail to obtainprecise values of fracture parameters. If the crack were modeled together with the wholecylinder, the resulting element size would be too small and the model would be too large.Along with the complexity of wall structure and material nonlinearity, it would demandtremendous computational cost. This restriction is resolved by a global-local FE analysisstrategy. The global model with coarse mesh is used to obtain the displacement solutionof the liner crack region. The local model of the region surrounding the crack is createdwith a very fine mesh. The boundary conditions of the local model are driven by thesolution of global analysis. The dimensions considered in the present analysis are based on a design typical ofthose described in literature [2]. The outer radius of the cylinder Rout is 0.229 m and theinner radius Rin is 0.217 m (Figure 1). The carbon/epoxy wrap consists of helical andhoop laminates resulting in a total composite shell thickness ( tc ) of 9 mm, and thethickness of the liner ( ta ) is 2.54 mm. The material properties are summarized in Tables1 and 2 [2, 23]. Study cases with various flaw sizes and proof pressures are summarizedin Table 3.3.1 Global Model For symmetry, one eighth of the cylinder is modeled, and symmetric boundaryconditions are imposed on the cut sides. The laminated composite wrap is modeled usinga doubly curved 8-node shell element and the liner by an 8-node solid brick element.Reduced integration is used to improve both computational efficiency and bendinganalysis accuracy. Figure 4 shows a schematic of the mesh for the whole cylinder model.
110.
99A finer mesh is used in the region, to which the local model will be applied. The wall isconstructed by tying the shell element to the brick element surface with an offset of a halfshell thickness. The lay-up of composite wrap ( [100 / 900 ]3 ) consists of six helical pliesalternated with three hoop plies (in Figure 4). The thickness of each helical ply is 0.55mm and each hoop ply is 1.9 mm in order to match the design stress ratio 0.8 (stress inthe helical layer/stress in the hoop layer). The material direction of the aluminum liner is1 in the hoop and 2 in the axial direction. Pressure loading is applied on the entire innersurface of the liner.3.2 Local Model To evaluate the fracture parameters for the axial crack, a local FE model is created fora small portion of the liner wall containing a crack (Figure 5). The size of the region isapproximately that of one element in the global model (marked in Figure 4). Thegeometry of the region is the same as the corresponding portion in the global model. Inconsideration of the crack symmetry, only half the crack is modeled. Quadraticcontinuum elements with 20 nodes (C3D20R in ABAQUS) are employed for betteraccuracy and better representation of the crack front curvature. The mesh density issignificantly higher than that for the global model, and the crack tip is surrounded bymany layers of elements. Singular continuum elements with a collapsed face are used tomodel the crack tip. For computation of K, 1/ r singularity is created using quarter-point nodes, where r is the distance to the crack tip. When the J-integral is evaluated, thenodes at crack tip are duplicated to create the combined 1/ r and 1/ r singularity forpower-law hardening.
111.
100 Figure 5 shows the local FE model of the region containing a crack. The bottom faceand the area below the crack front on the front face are applied with pressure loading.Boundary conditions of the top, back, and right faces are determined by displacementresults of the global analysis. Symmetric constraints are imposed on the left face and thearea above the crack front on the front face. The transfer of global analysis results to localanalysis is achieved using the sub-modeling procedure of ABAQUS software.3.3 Simulation Procedure The implementation scheme of the simulation procedure is illustrated in Figure 6. Theentire simulation is performed in three steps. The data swap between steps is assisted byABAQUS subroutines and the submodel technique. The procedure is executedautomatically by the control of Matlab software. Step 1: The autofrettage process is simulated in the global model by applying cyclicpressure loading. A stress state (marked as ‘ ’ in Figure 2) is selected and will beexported to the second step analysis as initial stress. Since the domain integral method inABAQUS does not consider the initial stress, the stress in the liner is chosen to be closeto zero in the selected stress state. The stress state selected for the model is recorded to afile using the ABAQUS user subroutine UVARM. Step 2: The displacement field needed for the submodel is computed from the globalmodel with a monotonic pressure loading applied from zero to operating pressures. Theautofrettage effect is introduced by applying the initial stresses in the model. From thefile created in Step 1, the initial stresses are read in using the ABAQUS user subroutineSIGINI.
112.
101 Step 3: The fracture parameters are extracted from the local model. The model isdriven by the boundary displacement computed from Step 2. Monotonic pressure loadingidentical to that in Step 2, is applied on the crack open face. Various material models areimplemented with a linear elastic model for K computation and an R-O model for J-integral evaluation.4. RESULTS AND DISCUSSION4.1 Autofrettage Process Simulation The far-field von-Mises stress distribution of the liner with four autofrettage levels isshown in Figure 7. The stresses are plotted as a function of pressure loading increment.The pressure load increases linearly to proof pressure in the first ten increments (Interval1), decreases to 0 in the next 10 increments (Interval 2), and rises back to operatingpressure in the last 10 increments (Interval 3). The yielding occurs during Interval 1, anda higher stress level is obtained by a higher proof pressure due to material hardening.When pressure returns to 0 at 20th increment, residual stresses are introduced bycompression of the composite wrap. Higher residual stresses occur at higher proofpressure. At the 30th increment, when it rises back to operating pressure, lower stressesremain in higher proof pressure cases. Figure 8 illustrates cyclic far-field stress-strain curves for the liner at four autofrettagelevels according to the loading sequence described in Figure 7. The stress/strain aligns inthe hoop direction which is perpendicular to the crack face. The deformation routes offour autofrettage levels are listed in the lower right corner of the figure. It can be seenthat higher compressive stress is introduced when higher proof pressure is applied, and
113.
102the opposite is taken for the tensile stresses. The variation of the introduced compressivestresses is proportional to proof pressure with the exception to the case of Pf =2.0 Po . Thereason is that the first three cases do not reach the compressive yielding strength andreturn linearly, and the last case yields at point 5 . Also, the Bauschinger effect can beobserved at point 5 , where the yielding stress is less than that at point 1 . Furthermore, thefour cases satisfy all constrains specified in section 2.1 and the selected stress fields areexported for the subsequent step analysis.4.2 Stress Intensity Factor (K) and J-integral In the present section, results along the crack front are normalized to θ as shown inthe inset in Figure 9. Stress intensity factor (K) and the J-integral along the crack frontare reported in Figures 9 and 10 respectively with four selected autofrettage levels. Thevalues of both K and the J-integral at a higher θ are much larger than those at a lower θ .This implies that the crack grows faster in the center so that the elliptic shape tends to bestretched closer to a circular shape. It can also be observed that the autofrettage processdramatically reduces the values of both K and the J-integral. Figures 11 and 12 plot K and the J-integral against the internal pressure loading. Thedotted horizontal lines mark the critical values of parameters (or fracture toughness)K c and Jc . At the beginning, values of fracture parameters are equal to zero, indicating thecrack is compressed to closure status by the composite wrap. With the internal pressureincreasing enough to overcome the compressive stress, the crack changes to the openingstatus. Value of stress intensity factor increases with loading linearly, while that of J-integral increases nonlinearly. Furthermore, the crack for case Pf =1.0 Po may stay inunstable growth condition since both the J-integral and K are above critical values.
114.
103 Figures 13 to 16 show K and the J-integral along the crack front with variousgeometric ratios when the proof pressure is equal to 1.5 times the operating pressure.Figures 13 and 14 show the results of cracks with same shape (depth/width ratio) butdifferent sizes (depth/thickness ratio). It can be seen that the crack size significantlyaffects fracture performance and fracture parameters of a larger crack have much highervalues. Figures 15 and 16 show the results of cracks with the same size and differentshapes. When the crack shape becomes closer to a circle (higher depth/width ratio), thecurve of fracture parameters becomes flatter. Crack growth speed along crack front isalmost same when a/c is equal to 0.75. However, when a/c is equal to 0.25, the center partof the crack grows much faster than two sides.4.3 Stress Field Characterization on the Crack Tip Vicinity Figure 17 shows the stress distribution around the crack tip of a typical loadingcondition. The stress is relaxed in the area under the crack tip near the free crack surface,while it is concentrated in the front of crack tip with an oblique angle where the plasticzone is formed. In Figure 18, three locations along the crack front curve, identified as A,B, and C, are selected to illustrate plastic zone shape and stress distribution. A planestrain like plastic zone is developed at A , takes transition around the B and turns into theshape of a typical plain stress plastic zone at C. Figure 19 shows the size of the plastic zone with four autofrettage levels at A and C.The critical plastic zone size is characterized by the radius rpc computed from Eq.(14) andmarked by dotted circles. It can be seen that large scale yielding occurs when Pf =1.0 P0 .The plastic zone grows out of the 2 rpc region, indicating fracture failure may occur byunstable crack growth. When Pf =1.25 P0 , the size of the plastic zone is large, compared
115.
104with dimensions of the crack length and the remaining ligament, which implies acontained yielding condition. When Pf =1.5 P0 , the plastic zone size is small enough forthe J-dominated stress field to be developed around the crack tip and the crack tipcondition can be characterized by the J-integral. Based on the ASTM standard, the caseof Pf =2.0 P0 can be safely characterized by one K parameter since the size of its plasticzone is at least fifteen times smaller than the other dimensions.5. CONCLUSIONS A comprehensive finite element model has been developed to predict the fracturebehavior of high pressure composite cylinders for hydrogen storage. The simulation ofthe autofrettage process is carried out in the global model. Plastic hardening andBauschinger effect are observed in the results. Both stress intensity factor (K) and the J-integral are computed along the crack front in the local model with consideration ofautofrettage influence and crack size effect. Results show that the autofrettage processsignificantly improves the cylinder fracture performance, and the smaller crack sizereduces the values of the fracture parameters dramatically. Shape and size of the plasticzone around the crack tip are examined. Fracture behavior is evaluated by observation ofthe plastic zone, and the corresponding parameter characterization is analyzed. Thedeveloped model and the proposed methodology can be used for design guidance toimprove cylinder fracture performance with consideration of autofrettage process, anddeveloping a fracture parameter database for fatigue life prediction.
116.
105 REFERENCES[1] D. Chapelle and D. Perreux, “Optimal Design of a Type 3 Hydrogen Vessel: Part I- Analytic Modeling of the Cylindrical Section,” International Journal of Hydrogen Energy, Vol.31, pp. 627–638, 2006.[2] F. Mitlitsky, A. H. Weisberg and B. Myers, “Vehicular Hydrogen Storage using Lightweight Tanks, ” Proceedings of the 2000 U.S.DOE Hydrogen Program Review, NREL/CP-570-28890, 2000.[3] H. Kobayashi, S. Sakai, M. Asano, K. Miyazaki, T. Nagasaki and Y. Takahashi, “Development of a Flaw Evaluation Handbook of the High Pressure Institute of Japan,” International Journal of Pressure Vessels and Piping, Vol.77, pp.929-936, 2000.[4] A. R. Shahani and S. E. Habibi, “Stress Intensity Factors in a Hollow Cylinder Containing a Circumferential Semi-elliptical Crack Subjected to Combined Loading,” International Journal of Fatigue, Vol. 29, pp.128-140, 2007.[5] J. H. Underwood, “Stress Intensity Factor for Internally Pressurized Thick Walled Cylinders,” ASTM STP, Vol. 513, pp. 59–70, 1972.[6] I. S. Raju and J. C. Newman, “An Empirical Stress Intensity Factor Equation for the Surface Crack,” Engineering Fracture Mechanics, Vol.15, pp. 185-192, 1981.[7] T. Fett, “Estimation of Stress Intensity Factors for Semi-elliptical Surface Cracks,” Engineering Fracture Mechanics, Vol. 66, pp.349-356, 2000.[8] J. R. Rice and N. Levy, “The Part-through Surface Crack in an Elastic Plate,” Journal of Applied Mechanics, ASME, Vol. 39, pp.185-194, 1972.[9] H. Lee and M. Parks, “Enhanced Elastic-plastic Line-spring Finite Element,” International Journal of Solids and Structures, Vol. 32, pp. 2393-2418, 1995.[10] I. S. Raju and J. C. Newman, “Stress-intensity Factor for Internal and External Surface Cracks in Cylindrical Vessels,” International Journal of Pressure Vessel Technology, Vol.104, pp.293-298, 1982.
117.
106[11] Y-J Kim, J-S Kim, Y-J Park and Y-J Kim, “Elastic–plastic Fracture Mechanics Method for Finite Internal Axial Surface Cracks in Cylinders,” Engineering Fracture Mechanics, Vol.71, pp.925-944, 2004.[12] A. Th. Diamantoudis and G. N. Labeas, “Stress Intensity Factors of Semi-elliptical Surface Cracks in Pressure Vessels by Global-local Finite Element Methodology,” Engineering Fracture Mechanics, Vol. 72, pp.1299-1312, 2005.[13] M. A. Guerrero, C. Betegon and J. Belzunce, “Fracture Analysis of a Pressure Vessel Made of High Strength Steel (HSS),” Engineering Failure Analysis, Vol.15, pp.208-219, 2008.[14] B. Su and G. S. Bhuyan, “The Fracture Behavior of the Aluminum Lined Hoop- wrapped Cylinders with Internal Axial Cracks,” International Journal of Pressure Vessels and Piping, Vol. 76, pp.251-257, 1999.[15] B. Su, Ch. Li and G. S. Bhuyan, “Comparison between Fractures Parameters of an All-aluminum Cylinder with Cracks under Different Deformation Conditions,” International Journal of Pressure Vessels and Piping, Vol.77, pp. 179-184, 2000.[16] A. R. Shahani and M. M. Kheirikhah, “Stress Intensity Factor Calculation of Steel- lined Hoop-wrapped Cylinders with Internal Semi-elliptical Circumferential Crack,” Engineering Fracture Mechanics, Vol.74, pp. 2004-2013, 2007.[17] M. Z. Kabir, “Finite Element Analysis of Composite Pressure Vessels with a Load Sharing Metallic Liner,” Composite Structures, Vol. 49, pp. 247-255, 2000.[18] G. W. Hunt, G. J. Lord and M. A. Peletier, “Cylindrical Shell Buckling: A Characterization of Localization and Periodicity,” Discrete and Continuous Dynamical Systems – Series B, Vol. 3, pp. 505-518, 2003.[19] T. L. Anderson, Fracture mechanics: Fundamentals and Applications. Boca Raton, Florida: CRC Press, 1995.[20] C. F. Shih and R. J. Asaro, “Elasto-plastic Analysis of Cracks on Bi-material Interfaces: Part I–Small Scale Yielding,” Journal of Applied Mechanics, ASME, Vol. 55, pp. 299–316, 1988.[21] ABAQUS version 6.7. Pawtucket, RI: Hibbitt, Karlsson & Sorensen Inc, 2007.
118.
107[22] B. Moran and C. F. Shih, “A General Treatment of Crack Tip, Contour Integrals,” International Journal of Fracture, Vol. 35, pp.295–310, 1987.[23] J. B. Jordon, M. F. Horstemeyer, K. Solanki and Y. Xue, “Damage and Stress State Influence on the Bauschinger Effect in Aluminum Alloys,” Mechanics of Materials Vol. 39, pp. 920–931 2007.
119.
108 LIST OF TABLESTable 1 Mechanical properties of carbon/epoxy compositeTable 2 Mechanical properties of Aluminum Alloy 7075-T651Table 3 Summary of study cases
120.
109 LIST OF FIGURESFigure 1 Schematic of hydrogen composite cylinderFigure 2 Diagram of autofrettage processFigure 3 Schematic of domain integral evaluationFigure 4 Global finite element modelFigure 5 Local finite element modelFigure 6 Implementation schemeFigure 7 von-Mises stress distribution in linerFigure 8 Cyclic stress-strain curves for various autofrettage levelsFigure 9 Stress intensity factor (K) along crack front for various autofrettage levelsFigure 10 J-integral along crack front for various autofrettage levelsFigure 11 Stress intensity factor (K) against pressure loading for various autofrettage levelsFigure 12 J-integral against pressure loading for various autofrettage levelsFigure 13 Stress intensity factor (K) along crack front with various geometric ratiosFigure 14 J-integral along crack front with various geometric ratiosFigure 15 Stress distribution of the crack front vicinityFigure 16 Transition of plastic zone shapes along crack frontFigure 17 Plastic zone shapes for various autofrettage levels
124.
113Figure 1 Schematic of hydrogen composite cylinder
125.
114 Proof pressure com D p 2 u Proof pressure state Operating pressure A 4 Operating pressure state t Composite 0 4 4 2 B (b)y 1 ucom Composite ultimatestress y Liner yielding stress C cy Liner compressive yielding stresst 4 u c Liner compressive stress 0 op t Liner tensile stress u Composite ultimatestrain op Operating strain cy 3c 4 p Applied pressure (a) Figure 2 Diagram of autofrettage process
126.
115 x2 V dS m crack front C C+ q x1 C x3 m Am outward normal S on the closed contourq virtual crack extension direction vector crack front Figure 3 Schematic of domain integral evaluation
136.
125 20 a/c=1/4 a/t a =0.75 18 Pf =1.5 P0 a/t a =0.50 16 K (MPam) 14 a/t a =0.25 12 10 8 6 0 10 20 30 40 50 60 70 80 90 (Degree)Figure 13 Stress intensity factor (K) along crack front with various geometric ratios
137.
126 5 a/c=1/4 a/t a =0.75 Pf =1.5 P0 4 a/t a =0.50 3 J (kPam) 2 a/t a =0.25 1 0 0 10 20 30 40 50 60 70 80 90 (Degree)Figure 14 J-integral along crack front with various geometric ratios
138.
127Figure 15 Stress distribution of the crack front vicinity
139.
128Plastic zone A B CFigure 16 Transition of plastic zone shapes along crack front
140.
129 1.5 Pf =1.0×Po 1 Length (mm) 2rpc Pf =1.25×Po 0.5 rpc Pf =1.5×Po Crack face Pf =2.0×Po 0 -1 -0.5 0 0.5 1 Length (mm) (a) At location A 1.5 Pf =1.0×Po 1 Length (mm) 2rpc 0.5 Pf =1.25×Po rpc Crack face Pf =1.5×Po Pf =2.0×Po 0 -1 -0.5 0 0.5 1 Length (mm) (b) At location CFigure 17 Plastic zone shapes for various autofrettage levels
141.
130 BIBLIOGRAPHY[1] Züttel, “Materials for Hydrogen Storage,” Materials Today, Vol.6, pp.24-33, 2003.[2] N. Takeichi, H. Senoh and T. Yokota, “‘Hybrid Hydrogen Storage Vessel’, a Novel High-pressure Hydrogen Storage Vessel Combined with Hydrogen Storage Material,” International Journal of Hydrogen Energy, Vol.28, pp.1121-1129, 2003.[3] E. David, “An Overview of Advanced Materials for Hydrogen Storage,” Journal of Materials Processing Technology, Vol.162-163, pp.169-177, 2005.[4] J. M. Lifshitz and H. Dayan, “Filament-wound Pressure Vessel with Thick Metal Liner,” Composite Structures, Vol.32, pp.313-323, 1995.[5] D. V. Rosato and C. S. Grove “Filament Winding, Its Development, Manufacture, Applications and Design,” New York: Interscience, 1964.[6] A. M. Shibley, “Filament winding, Handbook of Fiber-glass and Advanced Plastic Materials,” New York: Van Nostrand Reinhold, 1969.[7] S. T. Peters, W. D. Humphrey and R. F. Foral, “Filament Winding Composite Structure Fabrication,” Advancement of Material and Process Engineering, SAMPE International Business Office, 1991.[8] S. G. Lekhnitskii, “Theory of Elasticity of an Anisotropic Body,” Moscow: Mir Publishers, 1981.[9] J. Mistry, A. G. Gibson and Y-S. Wu, “Failure of Composite Cylinders under Combined External Pressure and Axial Loading,” Composite Structures, Vol.22, pp.193-200, 1992.[10] P. D. Soden, R. Kitching, P. C. Tse, M. J. Hinton and Y. Tsavalas, “Influence of Winding Angle on the Strength and Deformation of Filament-wound Composite Tubes Subjected to Uniaxial and Biaxial Loads,” Composites Science and Technology, Vol.46, pp.363–378, 1993.[11] M. F. S. Al-Khalil, P. D. Soden, R. Kitching and M. J. Hinton, “The Effects of Radial Stresses on the Strength of Thin-walled Filament Wound GRP Composite Pressure Cylinders,” International Journal of Mechanical Science,Vol.38, pp.97- 120, 1996.[12] P. M. Wild and G. W. Vickers, “Analysis of Filament-wound Cylindrical Sheels under Combined Centrifugal, Pressure and Axial Loading,” Composite Part A, Vol.28, pp.47-55, 1997.
142.
131[13] L. Parnas and N. Katırc, “Design of Fiber-reinforced Composite Pressure Vessels under Various Loading Conditions,” Composite Structure, Vol.58, pp.83-95, 2002.[14] H. Akcay and I. Kaynak, “Analysis of Multilayered Composite Cylinders under Thermal Loading,” Journal of Reinforced Plastics and Composites, Vol. 24, pp.1169-1179, 2005.[15] O. Sayman, “Analysis of Multi-layered Composite Cylinders under Hydrothermal Loading,” Composites: Part A, Vol.36, pp.923-933, 2005.[16] P. Y. Tabakov, “Design of Laminated Cylinders using Genetic Algorithm,” Journal of Applied Computer Science, Vol.8, pp.7-29, 2000.[17] P. Y. Tabakov and E. B. Summers, ”Lay-up Optimization of Multilayered Anisotropic Cylinders based on a 3-D Elasticity Solution,” Computers and Structures, Vol.84, pp.374-384, 2006.[18] D. Chapelle and D. Perreux, “Optimal Design of a Type 3 Hydrogen Vessel: Part I- Analytic Modeling of the Cylindrical Section,” International Journal of Hydrogen Energy, Vol.31, pp.627- 638, 2006.[19] S. V. Hoa, C. H. Yu and T. S. Sankar, “Analysis of Filament Wound Vessel Using Finite Elements,” Composite Structures, Vol. 3, pp.1-18, 1985.[20] J. Park, C. Hong, C-G. Kim and C-U. Kim, “Analysis of Filament Wound Composite Structures considering the Change of Winding Angles through the Thickness Direction,” Composite Structures, Vol. 55, pp.63-71, 2002.[21] M. Z. Kabir, “Finite Element Analysis of Composite Pressure Vessels with a Load Sharing Metallic Liner,” Composite Structures, Vol. 49, pp. 247-255, 2000.[22] H. T. Walter, P. S. Griffin and A. C. Jackson, “Design and Manufacture of a Composite Overwrapped Pressurant Tank Assembly,” 38th AIAA/ASME/SAE/ASEE Joint Propulsion Conference & Exhibit, Indianapolis, Indiana, AIAA 2002-4349, pp.1-12, 2002.[23] D. L. Gray and D. J. Moser, “Finite Element Analysis of a Composite Overwrapped Pressure Vessel,” 40th AIAA/ASME/SAE/ASEE Joint Propulsion Conference and Exhibit, Fort Lauderdale, Florida, AIAA 2004-3506, pp.1-15, 2004.[24] U. Kim, J. Kang, C. Hong and C. G. Kim, “Optimal Design of Filament Wound Structures under Internal Pressure based on the Semi-geodesic Path Algorithm,” Composite Structures, Vol. 67, pp.443-452, 2005.
143.
132[25] Y. D. Doh and C. S. Hong, “Progressive Failure Analysis for Filament Wound Pressure Vessel,” Journal of Reinforced Plastics and Composites, Vol.14, pp.1278- 1306, 1995.[26] C. Chamis, P. K. Gotsis and L. Minnetyan, “Progressive Fracture and Damage Tolerance of Composite Pressure Vessels,” Proceedings of The International Composites Expo, Session 5-C, pp.1-8, 1997.[27] L. Minnetyan, P. K. Gotsis and C. C. Chamis, “Progressive Damage and Fracture of Unstiffened and Stiffened Composite Pressure Vessels,” Journal of Reinforced Plastics and Composites, Vol.16, pp. 1711-1724, 1997.[28] J. Triplett, J. Patterson, J. R. Esslinger and J. Zalameda, “Impact Damage Evaluation of Stiffened Graphite Epoxy Cylinders,” American Institute of Aeronautics and Astronautics, AIAA-98-1787, pp.1809-1813, 1998.[29] R. Veys, A. Cederberg and J. Schimenti, “Fatigue Analysis Techniques for Composite Tankage with Plastically Operating Aluminum Liners,” AIAA, SAE, ASME, and ASEE, Joint Propulsion Conference, 27th, Sacramento, CA; United States; Vol.8, pp.24-26, 1991.[30] B. Su and G. S. Bhuyan, “Fracture Analyses on the All-metal Cylinders and the Metal-lined Hoop-wrapped Cylinders with Axial Cracks,” The International Journal of Pressure Vessels and Piping, Vol.76, pp.677-684, 1999.[31] C. Kaynak and O. Mat, “Uniaxial Fatigue Behavior of Filament-wound Glass- fiber/epoxy Composite Tubes,” Composites Science and Technology, Vol. 61, pp. 1833-1840, 2001.[32] N. Tarakc, L. Gemi and A. Yapici, “Fatigue Failure Behavior of Glass/epoxy ±55 Filament Wound Pipes under Internal Pressure,” Composites Science and Technology, Vol.65, pp.703-708, 2005.[33] A. R. Shahani and M. M. Kheirikhah, “Stress Intensity Factor Calculation of Steel- lined Hoop-wrapped Cylinders with Internal Semi-elliptical Circumferential Crack,” Engineering Fracture Mechanics, Vol.74, pp. 2004-2013, 2007.[34] M. A. Guerrero, C. Betegon and J. Belzunce, “Fracture Analysis of a Pressure Vessel Made of High Strength Steel (HSS),” Engineering Failure Analysis, Vol.15, pp.208-219, 2008.
144.
133 VITA Jianbing Hu was born on August 24th, 1979 in Xiaogan, Hubei, People’s RepublicChina. He joined Wuhan University of Technology, in Wuhan, China and obtained hisB.E. degree in Mechanical Engineering in 2000. He then joined Huazhong University ofScience & Technology, in Hubei, China in 2001 and obtained his M.S. degree inMechanical Engineering in 2004. Jianbing Hu later enrolled for his Ph.D. in MechanicalEngineering at Missouri S&T since August 2004. He has held the position of GraduateTeaching Assistant since August 2004 to May 2005 at Missouri S&T in the Departmentof Mechanical and Aerospace Engineering and also held the position of GraduateResearch Assistant since August 2004 to December 2008. He obtained his Ph.D. degreein Mechanical Engineering in Spring 2009 at Missouri S&T.
Be the first to comment